#------------------------------------------------------------------------------
#$Date: 2016-02-14 06:40:26 +0200 (Sun, 14 Feb 2016) $
#$Revision: 176432 $
#$URL: svn://www.crystallography.net/cod/cif/4/33/45/4334558.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4334558
loop_
_publ_author_name
'Partha Pratim Jana'
'Ryan Henderson'
'Bernd Harbrecht'
'Sven Lidin'
_publ_contact_author_address
;
CAS Chemical Centre
P O B 124
221 00 Lund
Sweden
;
_publ_contact_author_email       Partha.Jana@polymat.lth.se
_publ_contact_author_name        'Patha Pratim Jana'
_publ_section_title
;
 Site Preference and Ordering Induced by Au Substitution in the γ-Brass
 Related Complex Au-Cr-Zn Phases
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              4812
_journal_page_last               4818
_journal_paper_doi               10.1021/ic302244e
_journal_volume                  52
_journal_year                    2013
_chemical_formula_sum            'Au5.15 Cr4.73 Zn91.93'
_chemical_formula_weight         7270.10
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           216
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'F -4 2 3'
_symmetry_space_group_name_H-M   'F -4 3 m'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_audit_update_record
;
2012-09-21 # Formatted by publCIF
;
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   18.3653(7)
_cell_length_b                   18.3653(7)
_cell_length_c                   18.3653(7)
_cell_measurement_temperature    293(2)
_cell_volume                     6194.3(4)
_computing_cell_refinement       'IPDS software'
_computing_data_collection       'IPDS software'
_computing_data_reduction        'IPDS software/X-red'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'direct methods/SHELXS-97'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.985
_diffrn_measured_fraction_theta_max 0.985
_diffrn_measurement_device_type  IPDS(Stoe&Cie.)
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0512
_diffrn_reflns_av_sigmaI/netI    0.0171
_diffrn_reflns_limit_h_max       24
_diffrn_reflns_limit_h_min       -27
_diffrn_reflns_limit_k_max       27
_diffrn_reflns_limit_k_min       -27
_diffrn_reflns_limit_l_max       27
_diffrn_reflns_limit_l_min       -27
_diffrn_reflns_number            17464
_diffrn_reflns_theta_full        32.43
_diffrn_reflns_theta_max         32.43
_diffrn_reflns_theta_min         5.44
_exptl_absorpt_coefficient_mu    47.715
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   X-SHAPE
_exptl_crystal_density_diffrn    7.796
_exptl_crystal_description       'silvery with metallic luster'
_exptl_crystal_F_000             13114
_exptl_crystal_size_max          0.07
_exptl_crystal_size_mid          0.04
_exptl_crystal_size_min          0.03
_refine_diff_density_max         1.756
_refine_diff_density_min         -2.239
_refine_diff_density_rms         0.201
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.872(13)
_refine_ls_extinction_coef       0.000043(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.126
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     85
_refine_ls_number_reflns         1138
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.126
_refine_ls_R_factor_all          0.0282
_refine_ls_R_factor_gt           0.0273
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0077P)²+387.3427P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0535
_refine_ls_wR_factor_ref         0.0538
_reflns_number_gt                1114
_reflns_number_total             1138
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic302244e_si_001_08.cif
_cod_data_source_block           VII
_cod_original_sg_symbol_Hall     'F -4;2;3'
_cod_database_code               4334558
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'-x, y, -z'
'x, -y, -z'
'z, x, y'
'z, -x, -y'
'-z, -x, y'
'-z, x, -y'
'y, z, x'
'-y, z, -x'
'y, -z, -x'
'-y, -z, x'
'y, x, z'
'-y, -x, z'
'y, -x, -z'
'-y, x, -z'
'x, z, y'
'-x, z, -y'
'-x, -z, y'
'x, -z, -y'
'z, y, x'
'z, -y, -x'
'-z, y, -x'
'-z, -y, x'
'x, y+1/2, z+1/2'
'-x, -y+1/2, z+1/2'
'-x, y+1/2, -z+1/2'
'x, -y+1/2, -z+1/2'
'z, x+1/2, y+1/2'
'z, -x+1/2, -y+1/2'
'-z, -x+1/2, y+1/2'
'-z, x+1/2, -y+1/2'
'y, z+1/2, x+1/2'
'-y, z+1/2, -x+1/2'
'y, -z+1/2, -x+1/2'
'-y, -z+1/2, x+1/2'
'y, x+1/2, z+1/2'
'-y, -x+1/2, z+1/2'
'y, -x+1/2, -z+1/2'
'-y, x+1/2, -z+1/2'
'x, z+1/2, y+1/2'
'-x, z+1/2, -y+1/2'
'-x, -z+1/2, y+1/2'
'x, -z+1/2, -y+1/2'
'z, y+1/2, x+1/2'
'z, -y+1/2, -x+1/2'
'-z, y+1/2, -x+1/2'
'-z, -y+1/2, x+1/2'
'x+1/2, y, z+1/2'
'-x+1/2, -y, z+1/2'
'-x+1/2, y, -z+1/2'
'x+1/2, -y, -z+1/2'
'z+1/2, x, y+1/2'
'z+1/2, -x, -y+1/2'
'-z+1/2, -x, y+1/2'
'-z+1/2, x, -y+1/2'
'y+1/2, z, x+1/2'
'-y+1/2, z, -x+1/2'
'y+1/2, -z, -x+1/2'
'-y+1/2, -z, x+1/2'
'y+1/2, x, z+1/2'
'-y+1/2, -x, z+1/2'
'y+1/2, -x, -z+1/2'
'-y+1/2, x, -z+1/2'
'x+1/2, z, y+1/2'
'-x+1/2, z, -y+1/2'
'-x+1/2, -z, y+1/2'
'x+1/2, -z, -y+1/2'
'z+1/2, y, x+1/2'
'z+1/2, -y, -x+1/2'
'-z+1/2, y, -x+1/2'
'-z+1/2, -y, x+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1/2, z'
'-x+1/2, y+1/2, -z'
'x+1/2, -y+1/2, -z'
'z+1/2, x+1/2, y'
'z+1/2, -x+1/2, -y'
'-z+1/2, -x+1/2, y'
'-z+1/2, x+1/2, -y'
'y+1/2, z+1/2, x'
'-y+1/2, z+1/2, -x'
'y+1/2, -z+1/2, -x'
'-y+1/2, -z+1/2, x'
'y+1/2, x+1/2, z'
'-y+1/2, -x+1/2, z'
'y+1/2, -x+1/2, -z'
'-y+1/2, x+1/2, -z'
'x+1/2, z+1/2, y'
'-x+1/2, z+1/2, -y'
'-x+1/2, -z+1/2, y'
'x+1/2, -z+1/2, -y'
'z+1/2, y+1/2, x'
'z+1/2, -y+1/2, -x'
'-z+1/2, y+1/2, -x'
'-z+1/2, -y+1/2, x'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Zn10 Zn 0.0000 0.0000 0.0000 0.014(4) Uani 0.32(2) 24 d SP
Zn11 Zn 0.05454(10) 0.05454(10) 0.05454(10) 0.0204(9) Uani 0.710(11) 6 d SP
Au12 Au 0.913397(17) 0.913397(17) 0.913397(17) 0.01100(11) Uani 1 6 d S
Zn13 Zn 0.17620(18) 0.0000 0.0000 0.0427(7) Uani 1 4 d S
Zn15 Zn 0.15627(6) 0.15627(6) 0.02322(7) 0.0227(2) Uani 1 2 d S
Cr42 Cr 0.64871(7) 0.64871(7) 0.64871(7) 0.0086(4) Uani 1 6 d S
Zn43 Zn 0.64369(8) 0.2500 0.2500 0.0162(3) Uani 1 4 d S
Zn45 Zn 0.10718(5) 0.10718(5) 0.77504(6) 0.0197(2) Uani 1 2 d S
Zn30 Zn 0.5000 0.5000 0.5000 0.0233(9) Uani 1 24 d S
Zn32 Zn 0.41320(7) 0.41320(7) 0.41320(7) 0.0191(3) Uani 1 6 d S
Zn34 Zn 0.04821(4) 0.04821(4) 0.65268(7) 0.0175(2) Uani 1 2 d S
Zn35 Zn 0.19046(5) 0.19046(5) 0.51819(7) 0.0219(3) Uani 1 2 d S
Cr20 Cr 0.2500 0.2500 0.2500 0.0046(16) Uani 0.74(3) 24 d SP
Zn2B Zn 0.3113(15) 0.3113(15) 0.3113(15) 0.032(9) Uani 0.23(4) 6 d SP
Zn21 Zn 0.3206(3) 0.3474(10) 0.3206(3) 0.036(4) Uani 0.204(13) 2 d SP
Zn22 Zn 0.16664(8) 0.16664(8) 0.16664(8) 0.0229(7) Uani 0.901(11) 6 d SP
Zn23 Zn 0.08147(11) 0.2500 0.2500 0.0153(8) Uiso 0.231(7) 4 d SP
Au23 Au 0.08147(11) 0.2500 0.2500 0.0153(8) Uiso 0.193(7) 4 d SP
Zn24 Zn 0.3916(5) 0.2247(4) 0.2247(4) 0.030(3) Uiso 0.176(9) 2 d SP
Zn26 Zn 0.1113(8) 0.2703(7) 0.2703(7) 0.034(5) Uiso 0.109(10) 2 d SP
Zn25 Zn 0.07847(7) 0.07847(7) 0.26787(7) 0.0322(3) Uani 1 2 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cr Cr 0.3209 0.6236 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Au Au -2.0133 8.8022 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Zn11 Zn10 Zn11 109.5 . 4
Zn11 Zn10 Zn11 109.5 . 2
Zn11 Zn10 Zn11 109.5 4 2
Zn11 Zn10 Zn11 109.5 . 3
Zn11 Zn10 Zn11 109.5 4 3
Zn11 Zn10 Zn11 109.5 2 3
Zn11 Zn10 Au12 180.00(15) . 1_444
Zn11 Zn10 Au12 70.5 4 1_444
Zn11 Zn10 Au12 70.5 2 1_444
Zn11 Zn10 Au12 70.5 3 1_444
Zn11 Zn10 Au12 70.5 . 4_466
Zn11 Zn10 Au12 180.00(15) 4 4_466
Zn11 Zn10 Au12 70.5 2 4_466
Zn11 Zn10 Au12 70.5 3 4_466
Au12 Zn10 Au12 109.5 1_444 4_466
Zn11 Zn10 Au12 70.5 . 2_664
Zn11 Zn10 Au12 70.5 4 2_664
Zn11 Zn10 Au12 180.00(15) 2 2_664
Zn11 Zn10 Au12 70.5 3 2_664
Au12 Zn10 Au12 109.5 1_444 2_664
Au12 Zn10 Au12 109.5 4_466 2_664
Zn11 Zn10 Au12 70.5 . 3_646
Zn11 Zn10 Au12 70.5 4 3_646
Zn11 Zn10 Au12 70.5 2 3_646
Zn11 Zn10 Au12 180.00(15) 3 3_646
Au12 Zn10 Au12 109.5 1_444 3_646
Au12 Zn10 Au12 109.5 4_466 3_646
Au12 Zn10 Au12 109.5 2_664 3_646
Zn10 Zn11 Zn13 92.89(8) . 9
Zn10 Zn11 Zn13 92.89(8) . 5
Zn13 Zn11 Zn13 119.748(14) 9 5
Zn10 Zn11 Zn13 92.89(8) . .
Zn13 Zn11 Zn13 119.748(14) 9 .
Zn13 Zn11 Zn13 119.748(14) 5 .
Zn10 Zn11 Zn15 132.45(6) . .
Zn13 Zn11 Zn15 134.65(13) 9 .
Zn13 Zn11 Zn15 66.27(4) 5 .
Zn13 Zn11 Zn15 66.27(4) . .
Zn10 Zn11 Zn15 132.45(6) . 9
Zn13 Zn11 Zn15 66.27(4) 9 9
Zn13 Zn11 Zn15 134.65(13) 5 9
Zn13 Zn11 Zn15 66.27(4) . 9
Zn15 Zn11 Zn15 79.43(8) . 9
Zn10 Zn11 Zn15 132.45(6) . 5
Zn13 Zn11 Zn15 66.27(4) 9 5
Zn13 Zn11 Zn15 66.27(4) 5 5
Zn13 Zn11 Zn15 134.65(13) . 5
Zn15 Zn11 Zn15 79.43(8) . 5
Zn15 Zn11 Zn15 79.43(8) 9 5
Zn10 Zn11 Au12 72.55(7) . 2_664
Zn13 Zn11 Au12 165.44(14) 9 2_664
Zn13 Zn11 Au12 62.533(18) 5 2_664
Zn13 Zn11 Au12 62.533(18) . 2_664
Zn15 Zn11 Au12 59.91(3) . 2_664
Zn15 Zn11 Au12 123.67(5) 9 2_664
Zn15 Zn11 Au12 123.67(5) 5 2_664
Zn10 Zn11 Au12 72.55(7) . 3_646
Zn13 Zn11 Au12 62.533(18) 9 3_646
Zn13 Zn11 Au12 165.44(14) 5 3_646
Zn13 Zn11 Au12 62.533(18) . 3_646
Zn15 Zn11 Au12 123.67(5) . 3_646
Zn15 Zn11 Au12 59.91(3) 9 3_646
Zn15 Zn11 Au12 123.67(5) 5 3_646
Au12 Zn11 Au12 111.41(6) 2_664 3_646
Zn10 Zn11 Au12 72.55(7) . 4_466
Zn13 Zn11 Au12 62.533(18) 9 4_466
Zn13 Zn11 Au12 62.533(18) 5 4_466
Zn13 Zn11 Au12 165.44(14) . 4_466
Zn15 Zn11 Au12 123.67(5) . 4_466
Zn15 Zn11 Au12 123.67(5) 9 4_466
Zn15 Zn11 Au12 59.91(3) 5 4_466
Au12 Zn11 Au12 111.41(6) 2_664 4_466
Au12 Zn11 Au12 111.41(6) 3_646 4_466
Zn10 Zn11 Zn11 35.3 . 4
Zn13 Zn11 Zn11 109.24(7) 9 4
Zn13 Zn11 Zn11 109.24(7) 5 4
Zn13 Zn11 Zn11 57.63(8) . 4
Zn15 Zn11 Zn11 109.76(5) . 4
Zn15 Zn11 Zn11 109.76(5) 9 4
Zn15 Zn11 Zn11 167.72(6) 5 4
Au12 Zn11 Zn11 58.65(5) 2_664 4
Au12 Zn11 Zn11 58.65(5) 3_646 4
Au12 Zn11 Zn11 107.81(7) 4_466 4
Zn10 Zn11 Zn11 35.3 . 2
Zn13 Zn11 Zn11 57.63(8) 9 2
Zn13 Zn11 Zn11 109.24(7) 5 2
Zn13 Zn11 Zn11 109.24(7) . 2
Zn15 Zn11 Zn11 167.72(6) . 2
Zn15 Zn11 Zn11 109.76(5) 9 2
Zn15 Zn11 Zn11 109.76(5) 5 2
Au12 Zn11 Zn11 107.81(7) 2_664 2
Au12 Zn11 Zn11 58.65(5) 3_646 2
Au12 Zn11 Zn11 58.65(5) 4_466 2
Zn11 Zn11 Zn11 60.0 4 2
Zn45 Au12 Zn45 72.18(5) 10_656 6_566
Zn45 Au12 Zn45 72.18(5) 10_656 2_665
Zn45 Au12 Zn45 72.18(5) 6_566 2_665
Zn45 Au12 Zn15 65.01(3) 10_656 2_666
Zn45 Au12 Zn15 65.01(3) 6_566 2_666
Zn45 Au12 Zn15 126.23(5) 2_665 2_666
Zn45 Au12 Zn15 126.23(5) 10_656 10_666
Zn45 Au12 Zn15 65.01(3) 6_566 10_666
Zn45 Au12 Zn15 65.01(3) 2_665 10_666
Zn15 Au12 Zn15 118.686(14) 2_666 10_666
Zn45 Au12 Zn15 65.01(3) 10_656 6_666
Zn45 Au12 Zn15 126.23(5) 6_566 6_666
Zn45 Au12 Zn15 65.01(3) 2_665 6_666
Zn15 Au12 Zn15 118.686(14) 2_666 6_666
Zn15 Au12 Zn15 118.686(14) 10_666 6_666
Zn45 Au12 Zn11 112.44(6) 10_656 2_666
Zn45 Au12 Zn11 112.44(6) 6_566 2_666
Zn45 Au12 Zn11 174.06(7) 2_665 2_666
Zn15 Au12 Zn11 59.71(7) 2_666 2_666
Zn15 Au12 Zn11 113.00(4) 10_666 2_666
Zn15 Au12 Zn11 113.00(4) 6_666 2_666
Zn45 Au12 Zn11 174.06(7) 10_656 3_666
Zn45 Au12 Zn11 112.44(6) 6_566 3_666
Zn45 Au12 Zn11 112.44(6) 2_665 3_666
Zn15 Au12 Zn11 113.00(4) 2_666 3_666
Zn15 Au12 Zn11 59.71(7) 10_666 3_666
Zn15 Au12 Zn11 113.00(4) 6_666 3_666
Zn11 Au12 Zn11 62.70(11) 2_666 3_666
Zn45 Au12 Zn11 112.44(6) 10_656 4_666
Zn45 Au12 Zn11 174.06(7) 6_566 4_666
Zn45 Au12 Zn11 112.44(6) 2_665 4_666
Zn15 Au12 Zn11 113.00(4) 2_666 4_666
Zn15 Au12 Zn11 113.00(4) 10_666 4_666
Zn15 Au12 Zn11 59.71(7) 6_666 4_666
Zn11 Au12 Zn11 62.70(11) 2_666 4_666
Zn11 Au12 Zn11 62.70(11) 3_666 4_666
Zn45 Au12 Zn10 137.14(3) 10_656 1_666
Zn45 Au12 Zn10 137.14(3) 6_566 1_666
Zn45 Au12 Zn10 137.14(3) 2_665 1_666
Zn15 Au12 Zn10 96.63(4) 2_666 1_666
Zn15 Au12 Zn10 96.63(4) 10_666 1_666
Zn15 Au12 Zn10 96.63(4) 6_666 1_666
Zn11 Au12 Zn10 36.92(7) 2_666 1_666
Zn11 Au12 Zn10 36.92(7) 3_666 1_666
Zn11 Au12 Zn10 36.92(7) 4_666 1_666
Zn45 Au12 Zn13 123.75(4) 10_656 2_666
Zn45 Au12 Zn13 65.69(6) 6_566 2_666
Zn45 Au12 Zn13 123.75(4) 2_665 2_666
Zn15 Au12 Zn13 64.27(2) 2_666 2_666
Zn15 Au12 Zn13 64.27(2) 10_666 2_666
Zn15 Au12 Zn13 168.08(7) 6_666 2_666
Zn11 Au12 Zn13 57.38(5) 2_666 2_666
Zn11 Au12 Zn13 57.38(5) 3_666 2_666
Zn11 Au12 Zn13 108.38(9) 4_666 2_666
Zn10 Au12 Zn13 71.45(6) 1_666 2_666
Zn45 Au12 Zn13 65.69(6) 10_656 6_666
Zn45 Au12 Zn13 123.75(4) 6_566 6_666
Zn45 Au12 Zn13 123.75(4) 2_665 6_666
Zn15 Au12 Zn13 64.27(2) 2_666 6_666
Zn15 Au12 Zn13 168.08(7) 10_666 6_666
Zn15 Au12 Zn13 64.27(2) 6_666 6_666
Zn11 Au12 Zn13 57.38(5) 2_666 6_666
Zn11 Au12 Zn13 108.38(9) 3_666 6_666
Zn11 Au12 Zn13 57.38(5) 4_666 6_666
Zn10 Au12 Zn13 71.45(6) 1_666 6_666
Zn13 Au12 Zn13 110.38(5) 2_666 6_666
Zn25 Zn13 Zn25 100.89(12) 5 6
Zn25 Zn13 Zn11 161.93(12) 5 4
Zn25 Zn13 Zn11 97.18(8) 6 4
Zn25 Zn13 Zn11 97.18(8) 5 .
Zn25 Zn13 Zn11 161.93(12) 6 .
Zn11 Zn13 Zn11 64.74(16) 4 .
Zn25 Zn13 Au12 112.086(15) 5 2_664
Zn25 Zn13 Au12 112.086(15) 6 2_664
Zn11 Zn13 Au12 60.09(6) 4 2_664
Zn11 Zn13 Au12 60.09(6) . 2_664
Zn25 Zn13 Au12 112.086(15) 5 3_646
Zn25 Zn13 Au12 112.086(15) 6 3_646
Zn11 Zn13 Au12 60.09(6) 4 3_646
Zn11 Zn13 Au12 60.09(6) . 3_646
Au12 Zn13 Au12 107.62(11) 2_664 3_646
Zn25 Zn13 Zn45 78.75(5) 5 8_655
Zn25 Zn13 Zn45 78.75(5) 6 8_655
Zn11 Zn13 Zn45 104.99(5) 4 8_655
Zn11 Zn13 Zn45 104.99(5) . 8_655
Au12 Zn13 Zn45 54.02(3) 2_664 8_655
Au12 Zn13 Zn45 161.64(12) 3_646 8_655
Zn25 Zn13 Zn45 78.75(5) 5 7_655
Zn25 Zn13 Zn45 78.75(5) 6 7_655
Zn11 Zn13 Zn45 104.99(5) 4 7_655
Zn11 Zn13 Zn45 104.99(5) . 7_655
Au12 Zn13 Zn45 161.64(12) 2_664 7_655
Au12 Zn13 Zn45 54.02(3) 3_646 7_655
Zn45 Zn13 Zn45 144.33(13) 8_655 7_655
Zn25 Zn13 Zn15 133.97(9) 5 4
Zn25 Zn13 Zn15 57.67(3) 6 4
Zn11 Zn13 Zn15 57.83(7) 4 4
Zn11 Zn13 Zn15 108.72(11) . 4
Au12 Zn13 Zn15 113.76(8) 2_664 4
Au12 Zn13 Zn15 56.58(3) 3_646 4
Zn45 Zn13 Zn15 126.92(3) 8_655 4
Zn45 Zn13 Zn15 58.39(3) 7_655 4
Zn25 Zn13 Zn15 133.97(9) 5 11
Zn25 Zn13 Zn15 57.67(3) 6 11
Zn11 Zn13 Zn15 57.83(7) 4 11
Zn11 Zn13 Zn15 108.72(11) . 11
Au12 Zn13 Zn15 56.58(3) 2_664 11
Au12 Zn13 Zn15 113.76(8) 3_646 11
Zn45 Zn13 Zn15 58.39(3) 8_655 11
Zn45 Zn13 Zn15 126.92(3) 7_655 11
Zn15 Zn13 Zn15 72.43(5) 4 11
Zn25 Zn13 Zn15 57.67(3) 5 9
Zn25 Zn13 Zn15 133.97(9) 6 9
Zn11 Zn13 Zn15 108.72(11) 4 9
Zn11 Zn13 Zn15 57.83(7) . 9
Au12 Zn13 Zn15 113.76(8) 2_664 9
Au12 Zn13 Zn15 56.58(3) 3_646 9
Zn45 Zn13 Zn15 126.92(3) 8_655 9
Zn45 Zn13 Zn15 58.39(3) 7_655 9
Zn15 Zn13 Zn15 105.70(5) 4 9
Zn15 Zn13 Zn15 165.61(14) 11 9
Zn25 Zn13 Zn15 57.67(3) 5 .
Zn25 Zn13 Zn15 133.97(9) 6 .
Zn11 Zn13 Zn15 108.72(11) 4 .
Zn11 Zn13 Zn15 57.83(7) . .
Au12 Zn13 Zn15 56.58(3) 2_664 .
Au12 Zn13 Zn15 113.76(8) 3_646 .
Zn45 Zn13 Zn15 58.39(3) 8_655 .
Zn45 Zn13 Zn15 126.92(3) 7_655 .
Zn15 Zn13 Zn15 165.61(14) 4 .
Zn15 Zn13 Zn15 105.70(5) 11 .
Zn15 Zn13 Zn15 72.43(5) 9 .
Zn26 Zn15 Zn22 43.9(4) 84 .
Zn26 Zn15 Au23 16.6(4) 84 9
Zn22 Zn15 Au23 60.44(6) . 9
Zn26 Zn15 Zn23 16.6(4) 84 9
Zn22 Zn15 Zn23 60.44(6) . 9
Au23 Zn15 Zn23 0.00(8) 9 9
Zn26 Zn15 Zn25 68.44(9) 84 9
Zn22 Zn15 Zn25 66.99(4) . 9
Au23 Zn15 Zn25 72.52(5) 9 9
Zn23 Zn15 Zn25 72.52(5) 9 9
Zn26 Zn15 Zn25 68.44(9) 84 5
Zn22 Zn15 Zn25 66.99(4) . 5
Au23 Zn15 Zn25 72.52(5) 9 5
Zn23 Zn15 Zn25 72.52(5) 9 5
Zn25 Zn15 Zn25 131.59(9) 9 5
Zn26 Zn15 Zn11 127.4(4) 84 .
Zn22 Zn15 Zn11 83.56(8) . .
Au23 Zn15 Zn11 144.00(8) 9 .
Zn23 Zn15 Zn11 144.00(8) 9 .
Zn25 Zn15 Zn11 94.53(5) 9 .
Zn25 Zn15 Zn11 94.53(5) 5 .
Zn26 Zn15 Au12 172.2(4) 84 2_664
Zn22 Zn15 Au12 143.95(7) . 2_664
Au23 Zn15 Au12 155.61(8) 9 2_664
Zn23 Zn15 Au12 155.61(8) 9 2_664
Zn25 Zn15 Au12 112.88(5) 9 2_664
Zn25 Zn15 Au12 112.88(5) 5 2_664
Zn11 Zn15 Au12 60.39(6) . 2_664
Zn26 Zn15 Zn45 118.3(3) 84 8_655
Zn22 Zn15 Zn45 145.68(3) . 8_655
Au23 Zn15 Zn45 104.83(6) 9 8_655
Zn23 Zn15 Zn45 104.83(6) 9 8_655
Zn25 Zn15 Zn45 142.22(6) 9 8_655
Zn25 Zn15 Zn45 79.18(4) 5 8_655
Zn11 Zn15 Zn45 105.41(6) . 8_655
Au12 Zn15 Zn45 55.58(3) 2_664 8_655
Zn26 Zn15 Zn45 118.3(3) 84 11_565
Zn22 Zn15 Zn45 145.68(3) . 11_565
Au23 Zn15 Zn45 104.83(6) 9 11_565
Zn23 Zn15 Zn45 104.83(6) 9 11_565
Zn25 Zn15 Zn45 79.18(4) 9 11_565
Zn25 Zn15 Zn45 142.22(6) 5 11_565
Zn11 Zn15 Zn45 105.41(6) . 11_565
Au12 Zn15 Zn45 55.58(3) 2_664 11_565
Zn45 Zn15 Zn45 64.84(6) 8_655 11_565
Zn26 Zn15 Zn13 123.78(14) 84 5
Zn22 Zn15 Zn13 101.93(4) . 5
Au23 Zn15 Zn13 127.80(7) 9 5
Zn23 Zn15 Zn13 127.80(7) 9 5
Zn25 Zn15 Zn13 55.93(7) 9 5
Zn25 Zn15 Zn13 150.12(9) 5 5
Zn11 Zn15 Zn13 55.91(7) . 5
Au12 Zn15 Zn13 59.15(5) 2_664 5
Zn45 Zn15 Zn13 110.56(5) 8_655 5
Zn45 Zn15 Zn13 60.80(4) 11_565 5
Zn26 Zn15 Zn13 123.78(14) 84 .
Zn22 Zn15 Zn13 101.93(4) . .
Au23 Zn15 Zn13 127.80(7) 9 .
Zn23 Zn15 Zn13 127.80(7) 9 .
Zn25 Zn15 Zn13 150.12(9) 9 .
Zn25 Zn15 Zn13 55.93(7) 5 .
Zn11 Zn15 Zn13 55.91(7) . .
Au12 Zn15 Zn13 59.15(5) 2_664 .
Zn45 Zn15 Zn13 60.80(4) 8_655 .
Zn45 Zn15 Zn13 110.56(5) 11_565 .
Zn13 Zn15 Zn13 102.97(14) 5 .
Zn45 Cr42 Zn45 116.86(3) 57 29
Zn45 Cr42 Zn45 116.86(3) 57 73
Zn45 Cr42 Zn45 116.86(3) 29 73
Zn45 Cr42 Zn34 63.46(5) 57 57
Zn45 Cr42 Zn34 116.01(6) 29 57
Zn45 Cr42 Zn34 116.01(6) 73 57
Zn45 Cr42 Zn34 116.01(6) 57 29
Zn45 Cr42 Zn34 63.46(5) 29 29
Zn45 Cr42 Zn34 116.01(6) 73 29
Zn34 Cr42 Zn34 62.60(6) 57 29
Zn45 Cr42 Zn34 116.01(6) 57 73
Zn45 Cr42 Zn34 116.01(6) 29 73
Zn45 Cr42 Zn34 63.46(5) 73 73
Zn34 Cr42 Zn34 62.60(6) 57 73
Zn34 Cr42 Zn34 62.60(6) 29 73
Zn45 Cr42 Zn35 179.40(11) 57 57
Zn45 Cr42 Zn35 63.320(12) 29 57
Zn45 Cr42 Zn35 63.320(12) 73 57
Zn34 Cr42 Zn35 115.94(9) 57 57
Zn34 Cr42 Zn35 63.50(4) 29 57
Zn34 Cr42 Zn35 63.50(4) 73 57
Zn45 Cr42 Zn35 63.320(12) 57 29
Zn45 Cr42 Zn35 179.40(11) 29 29
Zn45 Cr42 Zn35 63.320(12) 73 29
Zn34 Cr42 Zn35 63.50(4) 57 29
Zn34 Cr42 Zn35 115.94(9) 29 29
Zn34 Cr42 Zn35 63.50(4) 73 29
Zn35 Cr42 Zn35 116.49(3) 57 29
Zn45 Cr42 Zn35 63.320(12) 57 73
Zn45 Cr42 Zn35 63.320(12) 29 73
Zn45 Cr42 Zn35 179.40(11) 73 73
Zn34 Cr42 Zn35 63.50(4) 57 73
Zn34 Cr42 Zn35 63.50(4) 29 73
Zn34 Cr42 Zn35 115.94(9) 73 73
Zn35 Cr42 Zn35 116.49(3) 57 73
Zn35 Cr42 Zn35 116.49(3) 29 73
Zn45 Cr42 Zn43 63.86(4) 57 81
Zn45 Cr42 Zn43 63.86(4) 29 81
Zn45 Cr42 Zn43 116.95(9) 73 81
Zn34 Cr42 Zn43 117.07(3) 57 81
Zn34 Cr42 Zn43 117.07(3) 29 81
Zn34 Cr42 Zn43 179.59(8) 73 81
Zn35 Cr42 Zn43 116.63(5) 57 81
Zn35 Cr42 Zn43 116.63(5) 29 81
Zn35 Cr42 Zn43 63.65(5) 73 81
Zn45 Cr42 Zn43 63.86(4) 57 25
Zn45 Cr42 Zn43 116.95(9) 29 25
Zn45 Cr42 Zn43 63.86(4) 73 25
Zn34 Cr42 Zn43 117.07(3) 57 25
Zn34 Cr42 Zn43 179.59(8) 29 25
Zn34 Cr42 Zn43 117.07(3) 73 25
Zn35 Cr42 Zn43 116.63(5) 57 25
Zn35 Cr42 Zn43 63.65(5) 29 25
Zn35 Cr42 Zn43 116.63(5) 73 25
Zn43 Cr42 Zn43 63.27(7) 81 25
Zn45 Cr42 Zn43 116.95(9) 57 53
Zn45 Cr42 Zn43 63.86(4) 29 53
Zn45 Cr42 Zn43 63.86(4) 73 53
Zn34 Cr42 Zn43 179.59(8) 57 53
Zn34 Cr42 Zn43 117.07(3) 29 53
Zn34 Cr42 Zn43 117.07(3) 73 53
Zn35 Cr42 Zn43 63.65(5) 57 53
Zn35 Cr42 Zn43 116.63(5) 29 53
Zn35 Cr42 Zn43 116.63(5) 73 53
Zn43 Cr42 Zn43 63.27(7) 81 53
Zn43 Cr42 Zn43 63.27(7) 25 53
Cr42 Zn43 Cr42 175.98(9) 4_566 25_544
Cr42 Zn43 Zn45 124.42(3) 4_566 81_545
Cr42 Zn43 Zn45 56.76(2) 25_544 81_545
Cr42 Zn43 Zn45 124.42(3) 4_566 49_554
Cr42 Zn43 Zn45 56.76(2) 25_544 49_554
Zn45 Zn43 Zn45 105.08(5) 81_545 49_554
Cr42 Zn43 Zn45 56.76(2) 4_566 59_565
Cr42 Zn43 Zn45 124.42(3) 25_544 59_565
Zn45 Zn43 Zn45 151.73(7) 81_545 59_565
Zn45 Zn43 Zn45 67.70(5) 49_554 59_565
Cr42 Zn43 Zn45 56.76(2) 4_566 76_556
Cr42 Zn43 Zn45 124.42(3) 25_544 76_556
Zn45 Zn43 Zn45 67.70(5) 81_545 76_556
Zn45 Zn43 Zn45 151.73(7) 49_554 76_556
Zn45 Zn43 Zn45 105.08(5) 59_565 76_556
Cr42 Zn43 Zn43 58.37(4) 4_566 10_656
Cr42 Zn43 Zn43 118.35(4) 25_544 10_656
Zn45 Zn43 Zn43 148.00(3) 81_545 10_656
Zn45 Zn43 Zn43 93.11(3) 49_554 10_656
Zn45 Zn43 Zn43 59.82(3) 59_565 10_656
Zn45 Zn43 Zn43 106.92(3) 76_556 10_656
Cr42 Zn43 Zn43 58.37(4) 4_566 54_565
Cr42 Zn43 Zn43 118.35(4) 25_544 54_565
Zn45 Zn43 Zn43 93.11(3) 81_545 54_565
Zn45 Zn43 Zn43 148.00(3) 49_554 54_565
Zn45 Zn43 Zn43 106.92(3) 59_565 54_565
Zn45 Zn43 Zn43 59.82(3) 76_556 54_565
Zn43 Zn43 Zn43 60.0 10_656 54_565
Cr42 Zn43 Zn43 118.35(4) 4_566 57_554
Cr42 Zn43 Zn43 58.37(4) 25_544 57_554
Zn45 Zn43 Zn43 59.82(3) 81_545 57_554
Zn45 Zn43 Zn43 106.92(3) 49_554 57_554
Zn45 Zn43 Zn43 148.00(3) 59_565 57_554
Zn45 Zn43 Zn43 93.11(3) 76_556 57_554
Zn43 Zn43 Zn43 90.0 10_656 57_554
Zn43 Zn43 Zn43 60.0 54_565 57_554
Cr42 Zn43 Zn43 118.35(4) 4_566 77_545
Cr42 Zn43 Zn43 58.37(4) 25_544 77_545
Zn45 Zn43 Zn43 106.92(3) 81_545 77_545
Zn45 Zn43 Zn43 59.82(3) 49_554 77_545
Zn45 Zn43 Zn43 93.11(3) 59_565 77_545
Zn45 Zn43 Zn43 148.00(3) 76_556 77_545
Zn43 Zn43 Zn43 60.0 10_656 77_545
Zn43 Zn43 Zn43 90.0 54_565 77_545
Zn43 Zn43 Zn43 60.0 57_554 77_545
Cr42 Zn43 Zn35 125.87(6) 4_566 5
Cr42 Zn43 Zn35 58.15(4) 25_544 5
Zn45 Zn43 Zn35 59.13(3) 81_545 5
Zn45 Zn43 Zn35 59.13(3) 49_554 5
Zn45 Zn43 Zn35 96.18(4) 59_565 5
Zn45 Zn43 Zn35 96.18(4) 76_556 5
Zn43 Zn43 Zn35 149.970(1) 10_656 5
Zn43 Zn43 Zn35 149.970(1) 54_565 5
Zn43 Zn43 Zn35 107.97(3) 57_554 5
Zn43 Zn43 Zn35 107.97(3) 77_545 5
Cr42 Zn43 Zn35 58.15(4) 4_566 30
Cr42 Zn43 Zn35 125.87(6) 25_544 30
Zn45 Zn43 Zn35 96.18(4) 81_545 30
Zn45 Zn43 Zn35 96.18(4) 49_554 30
Zn45 Zn43 Zn35 59.13(3) 59_565 30
Zn45 Zn43 Zn35 59.13(3) 76_556 30
Zn43 Zn43 Zn35 107.97(3) 10_656 30
Zn43 Zn43 Zn35 107.97(3) 54_565 30
Zn43 Zn43 Zn35 149.970(1) 57_554 30
Zn43 Zn43 Zn35 149.970(1) 77_545 30
Zn35 Zn43 Zn35 67.72(6) 5 30
Cr42 Zn45 Au12 166.94(8) 73_445 2_665
Cr42 Zn45 Zn34 59.21(6) 73_445 .
Au12 Zn45 Zn34 133.85(6) 2_665 .
Cr42 Zn45 Zn35 59.63(4) 73_445 33_545
Au12 Zn45 Zn35 123.53(4) 2_665 33_545
Zn34 Zn45 Zn35 60.89(4) . 33_545
Cr42 Zn45 Zn35 59.63(4) 73_445 53_455
Au12 Zn45 Zn35 123.53(4) 2_665 53_455
Zn34 Zn45 Zn35 60.89(4) . 53_455
Zn35 Zn45 Zn35 110.39(7) 33_545 53_455
Cr42 Zn45 Zn43 59.38(5) 73_445 29_545
Au12 Zn45 Zn43 109.78(4) 2_665 29_545
Zn34 Zn45 Zn43 109.83(4) . 29_545
Zn35 Zn45 Zn43 60.98(4) 33_545 29_545
Zn35 Zn45 Zn43 109.90(5) 53_455 29_545
Cr42 Zn45 Zn43 59.38(5) 73_445 49_455
Au12 Zn45 Zn43 109.78(4) 2_665 49_455
Zn34 Zn45 Zn43 109.83(4) . 49_455
Zn35 Zn45 Zn43 109.90(5) 33_545 49_455
Zn35 Zn45 Zn43 60.98(4) 53_455 49_455
Zn43 Zn45 Zn43 60.36(7) 29_545 49_455
Cr42 Zn45 Zn15 123.85(3) 73_445 8_556
Au12 Zn45 Zn15 59.41(3) 2_665 8_556
Zn34 Zn45 Zn15 99.03(4) . 8_556
Zn35 Zn45 Zn15 155.91(6) 33_545 8_556
Zn35 Zn45 Zn15 64.61(4) 53_455 8_556
Zn43 Zn45 Zn15 143.00(5) 29_545 8_556
Zn43 Zn45 Zn15 88.69(4) 49_455 8_556
Cr42 Zn45 Zn15 123.85(3) 73_445 11_556
Au12 Zn45 Zn15 59.41(3) 2_665 11_556
Zn34 Zn45 Zn15 99.03(4) . 11_556
Zn35 Zn45 Zn15 64.61(4) 33_545 11_556
Zn35 Zn45 Zn15 155.91(6) 53_455 11_556
Zn43 Zn45 Zn15 88.69(4) 29_545 11_556
Zn43 Zn45 Zn15 143.00(5) 49_455 11_556
Zn15 Zn45 Zn15 109.57(7) 8_556 11_556
Cr42 Zn45 Zn13 132.77(9) 73_445 10_556
Au12 Zn45 Zn13 60.29(7) 2_665 10_556
Zn34 Zn45 Zn13 73.56(7) . 10_556
Zn35 Zn45 Zn13 98.55(5) 33_545 10_556
Zn35 Zn45 Zn13 98.55(5) 53_455 10_556
Zn43 Zn45 Zn13 149.16(3) 29_545 10_556
Zn43 Zn45 Zn13 149.16(3) 49_455 10_556
Zn15 Zn45 Zn13 60.81(4) 8_556 10_556
Zn15 Zn45 Zn13 60.81(4) 11_556 10_556
Cr42 Zn45 Zn45 115.49(5) 73_445 11_566
Au12 Zn45 Zn45 53.91(2) 2_665 11_566
Zn34 Zn45 Zn45 149.985(1) . 11_566
Zn35 Zn45 Zn45 145.82(4) 33_545 11_566
Zn35 Zn45 Zn45 90.36(4) 53_455 11_566
Zn43 Zn45 Zn45 86.89(3) 29_545 11_566
Zn43 Zn45 Zn45 56.15(2) 49_455 11_566
Zn15 Zn45 Zn45 57.58(3) 8_556 11_566
Zn15 Zn45 Zn45 106.31(3) 11_556 11_566
Zn13 Zn45 Zn45 105.04(6) 10_556 11_566
Cr42 Zn45 Zn45 115.49(5) 73_445 8_656
Au12 Zn45 Zn45 53.91(2) 2_665 8_656
Zn34 Zn45 Zn45 149.985(1) . 8_656
Zn35 Zn45 Zn45 90.36(4) 33_545 8_656
Zn35 Zn45 Zn45 145.82(4) 53_455 8_656
Zn43 Zn45 Zn45 56.15(2) 29_545 8_656
Zn43 Zn45 Zn45 86.89(3) 49_455 8_656
Zn15 Zn45 Zn45 106.31(3) 8_556 8_656
Zn15 Zn45 Zn45 57.58(3) 11_556 8_656
Zn13 Zn45 Zn45 105.04(6) 10_556 8_656
Zn45 Zn45 Zn45 60.0 11_566 8_656
Zn32 Zn30 Zn32 109.5 . 4_566
Zn32 Zn30 Zn32 109.5 . 2_665
Zn32 Zn30 Zn32 109.5 4_566 2_665
Zn32 Zn30 Zn32 109.5 . 3_656
Zn32 Zn30 Zn32 109.5 4_566 3_656
Zn32 Zn30 Zn32 109.5 2_665 3_656
Zn32 Zn30 Zn34 149.33(2) . 57
Zn32 Zn30 Zn34 58.185(6) 4_566 57
Zn32 Zn30 Zn34 58.185(6) 2_665 57
Zn32 Zn30 Zn34 101.20(2) 3_656 57
Zn32 Zn30 Zn34 149.33(2) . 73
Zn32 Zn30 Zn34 58.185(6) 4_566 73
Zn32 Zn30 Zn34 101.20(2) 2_665 73
Zn32 Zn30 Zn34 58.185(6) 3_656 73
Zn34 Zn30 Zn34 52.43(3) 57 73
Zn32 Zn30 Zn34 149.33(2) . 29
Zn32 Zn30 Zn34 101.20(2) 4_566 29
Zn32 Zn30 Zn34 58.185(6) 2_665 29
Zn32 Zn30 Zn34 58.185(6) 3_656 29
Zn34 Zn30 Zn34 52.43(3) 57 29
Zn34 Zn30 Zn34 52.43(3) 73 29
Zn32 Zn30 Zn34 101.20(2) . 58
Zn32 Zn30 Zn34 58.185(6) 4_566 58
Zn32 Zn30 Zn34 58.185(6) 2_665 58
Zn32 Zn30 Zn34 149.33(2) 3_656 58
Zn34 Zn30 Zn34 48.13(4) 57 58
Zn34 Zn30 Zn34 94.769(8) 73 58
Zn34 Zn30 Zn34 94.769(8) 29 58
Zn32 Zn30 Zn34 101.20(2) . 74
Zn32 Zn30 Zn34 58.185(6) 4_566 74
Zn32 Zn30 Zn34 149.33(2) 2_665 74
Zn32 Zn30 Zn34 58.185(6) 3_656 74
Zn34 Zn30 Zn34 94.769(8) 57 74
Zn34 Zn30 Zn34 48.13(4) 73 74
Zn34 Zn30 Zn34 94.769(8) 29 74
Zn34 Zn30 Zn34 116.321(13) 58 74
Zn32 Zn30 Zn34 101.20(2) . 30
Zn32 Zn30 Zn34 149.33(2) 4_566 30
Zn32 Zn30 Zn34 58.185(6) 2_665 30
Zn32 Zn30 Zn34 58.185(6) 3_656 30
Zn34 Zn30 Zn34 94.769(8) 57 30
Zn34 Zn30 Zn34 94.769(8) 73 30
Zn34 Zn30 Zn34 48.13(4) 29 30
Zn34 Zn30 Zn34 116.322(13) 58 30
Zn34 Zn30 Zn34 116.322(13) 74 30
Zn32 Zn30 Zn34 58.185(6) . 60_565
Zn32 Zn30 Zn34 101.20(2) 4_566 60_565
Zn32 Zn30 Zn34 149.33(2) 2_665 60_565
Zn32 Zn30 Zn34 58.185(6) 3_656 60_565
Zn34 Zn30 Zn34 146.48(3) 57 60_565
Zn34 Zn30 Zn34 94.769(8) 73 60_565
Zn34 Zn30 Zn34 116.322(13) 29 60_565
Zn34 Zn30 Zn34 146.48(3) 58 60_565
Zn34 Zn30 Zn34 52.43(3) 74 60_565
Zn34 Zn30 Zn34 94.769(8) 30 60_565
Zn32 Zn30 Zn34 58.185(6) . 31_655
Zn32 Zn30 Zn34 58.185(6) 4_566 31_655
Zn32 Zn30 Zn34 149.33(2) 2_665 31_655
Zn32 Zn30 Zn34 101.20(2) 3_656 31_655
Zn34 Zn30 Zn34 116.322(13) 57 31_655
Zn34 Zn30 Zn34 94.769(8) 73 31_655
Zn34 Zn30 Zn34 146.48(3) 29 31_655
Zn34 Zn30 Zn34 94.769(8) 58 31_655
Zn34 Zn30 Zn34 52.43(3) 74 31_655
Zn34 Zn30 Zn34 146.48(3) 30 31_655
Zn34 Zn30 Zn34 52.43(3) 60_565 31_655
Zn25 Zn32 Zn25 96.35(8) 58 30
Zn25 Zn32 Zn25 96.35(8) 58 74
Zn25 Zn32 Zn25 96.35(8) 30 74
Zn25 Zn32 Zn21 67.9(4) 58 .
Zn25 Zn32 Zn21 55.39(18) 30 .
Zn25 Zn32 Zn21 55.39(18) 74 .
Zn25 Zn32 Zn21 55.39(18) 58 9
Zn25 Zn32 Zn21 67.9(4) 30 9
Zn25 Zn32 Zn21 55.39(18) 74 9
Zn21 Zn32 Zn21 14.8(7) . 9
Zn25 Zn32 Zn21 55.39(18) 58 5
Zn25 Zn32 Zn21 55.39(18) 30 5
Zn25 Zn32 Zn21 67.9(4) 74 5
Zn21 Zn32 Zn21 14.8(7) . 5
Zn21 Zn32 Zn21 14.8(7) 9 5
Zn25 Zn32 Zn30 120.63(6) 58 .
Zn25 Zn32 Zn30 120.63(6) 30 .
Zn25 Zn32 Zn30 120.63(6) 74 .
Zn21 Zn32 Zn30 171.4(4) . .
Zn21 Zn32 Zn30 171.4(4) 9 .
Zn21 Zn32 Zn30 171.4(4) 5 .
Zn25 Zn32 Zn34 60.84(4) 58 59_565
Zn25 Zn32 Zn34 151.36(3) 30 59_565
Zn25 Zn32 Zn34 102.86(2) 74 59_565
Zn21 Zn32 Zn34 121.1(3) . 59_565
Zn21 Zn32 Zn34 106.3(4) 9 59_565
Zn21 Zn32 Zn34 113.16(6) 5 59_565
Zn30 Zn32 Zn34 66.36(4) . 59_565
Zn25 Zn32 Zn34 60.84(4) 58 60_565
Zn25 Zn32 Zn34 102.86(2) 30 60_565
Zn25 Zn32 Zn34 151.36(3) 74 60_565
Zn21 Zn32 Zn34 121.1(3) . 60_565
Zn21 Zn32 Zn34 113.16(6) 9 60_565
Zn21 Zn32 Zn34 106.3(4) 5 60_565
Zn30 Zn32 Zn34 66.36(4) . 60_565
Zn34 Zn32 Zn34 52.16(4) 59_565 60_565
Zn25 Zn32 Zn34 151.36(3) 58 32_655
Zn25 Zn32 Zn34 60.84(4) 30 32_655
Zn25 Zn32 Zn34 102.86(2) 74 32_655
Zn21 Zn32 Zn34 106.3(4) . 32_655
Zn21 Zn32 Zn34 121.1(3) 9 32_655
Zn21 Zn32 Zn34 113.16(6) 5 32_655
Zn30 Zn32 Zn34 66.36(4) . 32_655
Zn34 Zn32 Zn34 132.65(9) 59_565 32_655
Zn34 Zn32 Zn34 105.00(5) 60_565 32_655
Zn25 Zn32 Zn34 102.86(2) 58 31_655
Zn25 Zn32 Zn34 60.84(4) 30 31_655
Zn25 Zn32 Zn34 151.36(3) 74 31_655
Zn21 Zn32 Zn34 113.16(6) . 31_655
Zn21 Zn32 Zn34 121.1(3) 9 31_655
Zn21 Zn32 Zn34 106.3(4) 5 31_655
Zn30 Zn32 Zn34 66.36(4) . 31_655
Zn34 Zn32 Zn34 105.00(5) 59_565 31_655
Zn34 Zn32 Zn34 56.88(5) 60_565 31_655
Zn34 Zn32 Zn34 52.16(4) 32_655 31_655
Zn25 Zn32 Zn34 151.36(3) 58 75_556
Zn25 Zn32 Zn34 102.86(2) 30 75_556
Zn25 Zn32 Zn34 60.84(4) 74 75_556
Zn21 Zn32 Zn34 106.3(4) . 75_556
Zn21 Zn32 Zn34 113.16(6) 9 75_556
Zn21 Zn32 Zn34 121.1(3) 5 75_556
Zn30 Zn32 Zn34 66.36(4) . 75_556
Zn34 Zn32 Zn34 105.00(5) 59_565 75_556
Zn34 Zn32 Zn34 132.65(9) 60_565 75_556
Zn34 Zn32 Zn34 56.88(5) 32_655 75_556
Zn34 Zn32 Zn34 105.00(5) 31_655 75_556
Zn34 Zn34 Cr42 178.40(4) 2 73_445
Zn34 Zn34 Zn34 120.0 2 33_545
Cr42 Zn34 Zn34 58.70(3) 73_445 33_545
Zn34 Zn34 Zn34 120.0 2 53_455
Cr42 Zn34 Zn34 58.70(3) 73_445 53_455
Zn34 Zn34 Zn34 60.0 33_545 53_455
Zn34 Zn34 Zn45 124.28(4) 2 .
Cr42 Zn34 Zn45 57.32(4) 73_445 .
Zn34 Zn34 Zn45 107.62(3) 33_545 .
Zn34 Zn34 Zn45 107.62(3) 53_455 .
Zn34 Zn34 Zn35 121.89(3) 2 33_545
Cr42 Zn34 Zn35 58.60(3) 73_445 33_545
Zn34 Zn34 Zn35 108.61(3) 33_545 33_545
Zn34 Zn34 Zn35 60.54(3) 53_455 33_545
Zn45 Zn34 Zn35 59.65(3) . 33_545
Zn34 Zn34 Zn35 121.89(3) 2 53_455
Cr42 Zn34 Zn35 58.60(3) 73_445 53_455
Zn34 Zn34 Zn35 60.54(3) 33_545 53_455
Zn34 Zn34 Zn35 108.61(3) 53_455 53_455
Zn45 Zn34 Zn35 59.65(3) . 53_455
Zn35 Zn34 Zn35 108.38(7) 33_545 53_455
Zn34 Zn34 Zn25 63.46(2) 2 4_556
Cr42 Zn34 Zn25 117.47(3) 73_445 4_556
Zn34 Zn34 Zn25 162.82(4) 33_545 4_556
Zn34 Zn34 Zn25 103.18(4) 53_455 4_556
Zn45 Zn34 Zn25 79.71(4) . 4_556
Zn35 Zn34 Zn25 61.00(3) 33_545 4_556
Zn35 Zn34 Zn25 134.03(6) 53_455 4_556
Zn34 Zn34 Zn25 63.46(2) 2 3_556
Cr42 Zn34 Zn25 117.47(3) 73_445 3_556
Zn34 Zn34 Zn25 103.18(4) 33_545 3_556
Zn34 Zn34 Zn25 162.82(4) 53_455 3_556
Zn45 Zn34 Zn25 79.71(4) . 3_556
Zn35 Zn34 Zn25 134.03(6) 33_545 3_556
Zn35 Zn34 Zn25 61.00(3) 53_455 3_556
Zn25 Zn34 Zn25 93.34(8) 4_556 3_556
Zn34 Zn34 Zn32 63.92(2) 2 75_546
Cr42 Zn34 Zn32 115.31(3) 73_445 75_546
Zn34 Zn34 Zn32 108.37(4) 33_545 75_546
Zn34 Zn34 Zn32 61.56(2) 53_455 75_546
Zn45 Zn34 Zn32 126.77(4) . 75_546
Zn35 Zn34 Zn32 72.38(4) 33_545 75_546
Zn35 Zn34 Zn32 168.77(6) 53_455 75_546
Zn25 Zn34 Zn32 56.57(5) 4_556 75_546
Zn25 Zn34 Zn32 126.90(4) 3_556 75_546
Zn34 Zn34 Zn32 63.92(2) 2 76_456
Cr42 Zn34 Zn32 115.31(3) 73_445 76_456
Zn34 Zn34 Zn32 61.56(2) 33_545 76_456
Zn34 Zn34 Zn32 108.37(4) 53_455 76_456
Zn45 Zn34 Zn32 126.77(4) . 76_456
Zn35 Zn34 Zn32 168.77(6) 33_545 76_456
Zn35 Zn34 Zn32 72.38(4) 53_455 76_456
Zn25 Zn34 Zn32 126.90(4) 4_556 76_456
Zn25 Zn34 Zn32 56.57(5) 3_556 76_456
Zn32 Zn34 Zn32 104.64(8) 75_546 76_456
Zn34 Zn34 Zn30 65.94(2) 2 73_445
Cr42 Zn34 Zn30 112.47(5) 73_445 73_445
Zn34 Zn34 Zn30 63.783(17) 33_545 73_445
Zn34 Zn34 Zn30 63.783(17) 53_455 73_445
Zn45 Zn34 Zn30 169.79(5) . 73_445
Zn35 Zn34 Zn30 116.43(3) 33_545 73_445
Zn35 Zn34 Zn30 116.43(3) 53_455 73_445
Zn25 Zn34 Zn30 107.05(4) 4_556 73_445
Zn25 Zn34 Zn30 107.05(4) 3_556 73_445
Zn32 Zn34 Zn30 55.45(4) 75_546 73_445
Zn32 Zn34 Zn30 55.45(4) 76_456 73_445
Au23 Zn35 Zn23 0.00(6) 58 58
Au23 Zn35 Zn24 19.3(2) 58 9
Zn23 Zn35 Zn24 19.3(2) 58 9
Au23 Zn35 Cr42 164.14(8) 58 73_445
Zn23 Zn35 Cr42 164.14(8) 58 73_445
Zn24 Zn35 Cr42 176.6(3) 9 73_445
Au23 Zn35 Zn45 117.01(4) 58 33_545
Zn23 Zn35 Zn45 117.01(4) 58 33_545
Zn24 Zn35 Zn45 123.92(7) 9 33_545
Cr42 Zn35 Zn45 57.04(4) 73_445 33_545
Au23 Zn35 Zn45 117.01(4) 58 53_455
Zn23 Zn35 Zn45 117.01(4) 58 53_455
Zn24 Zn35 Zn45 123.92(7) 9 53_455
Cr42 Zn35 Zn45 57.05(4) 73_445 53_455
Zn45 Zn35 Zn45 106.28(7) 33_545 53_455
Au23 Zn35 Zn34 134.40(5) 58 33_545
Zn23 Zn35 Zn34 134.40(5) 58 33_545
Zn24 Zn35 Zn34 119.3(2) 9 33_545
Cr42 Zn35 Zn34 57.90(5) 73_445 33_545
Zn45 Zn35 Zn34 59.46(4) 33_545 33_545
Zn45 Zn35 Zn34 106.19(6) 53_455 33_545
Au23 Zn35 Zn34 134.40(5) 58 53_455
Zn23 Zn35 Zn34 134.40(5) 58 53_455
Zn24 Zn35 Zn34 119.3(2) 9 53_455
Cr42 Zn35 Zn34 57.90(5) 73_445 53_455
Zn45 Zn35 Zn34 106.19(6) 33_545 53_455
Zn45 Zn35 Zn34 59.46(4) 53_455 53_455
Zn34 Zn35 Zn34 58.92(6) 33_545 53_455
Au23 Zn35 Zn43 105.94(6) 58 9
Zn23 Zn35 Zn43 105.94(6) 58 9
Zn24 Zn35 Zn43 125.2(2) 9 9
Cr42 Zn35 Zn43 58.20(6) 73_445 9
Zn45 Zn35 Zn43 59.90(4) 33_545 9
Zn45 Zn35 Zn43 59.90(4) 53_455 9
Zn34 Zn35 Zn43 107.83(5) 33_545 9
Zn34 Zn35 Zn43 107.83(5) 53_455 9
Au23 Zn35 Zn25 74.24(5) 58 35
Zn23 Zn35 Zn25 74.24(5) 58 35
Zn24 Zn35 Zn25 61.84(15) 9 35
Cr42 Zn35 Zn25 116.09(6) 73_445 35
Zn45 Zn35 Zn25 79.26(5) 33_545 35
Zn45 Zn35 Zn25 160.89(6) 53_455 35
Zn34 Zn35 Zn25 60.26(4) 33_545 35
Zn34 Zn35 Zn25 101.50(5) 53_455 35
Zn43 Zn35 Zn25 134.63(4) 9 35
Au23 Zn35 Zn25 74.24(5) 58 56
Zn23 Zn35 Zn25 74.24(5) 58 56
Zn24 Zn35 Zn25 61.84(15) 9 56
Cr42 Zn35 Zn25 116.09(6) 73_445 56
Zn45 Zn35 Zn25 160.89(6) 33_545 56
Zn45 Zn35 Zn25 79.26(5) 53_455 56
Zn34 Zn35 Zn25 101.50(5) 33_545 56
Zn34 Zn35 Zn25 60.26(4) 53_455 56
Zn43 Zn35 Zn25 134.63(4) 9 56
Zn25 Zn35 Zn25 89.98(8) 35 56
Au23 Zn35 Zn26 12.7(3) 58 35
Zn23 Zn35 Zn26 12.7(3) 58 35
Zn24 Zn35 Zn26 16.0(3) 9 35
Cr42 Zn35 Zn26 166.4(3) 73_445 35
Zn45 Zn35 Zn26 129.6(3) 33_545 35
Zn45 Zn35 Zn26 110.2(3) 53_455 35
Zn34 Zn35 Zn26 135.1(2) 33_545 35
Zn34 Zn35 Zn26 122.0(3) 53_455 35
Zn43 Zn35 Zn26 112.70(18) 9 35
Zn25 Zn35 Zn26 77.5(3) 35 35
Zn25 Zn35 Zn26 61.7(3) 56 35
Zn2B Cr20 Zn2B 109.471(8) . 28
Zn2B Cr20 Zn2B 109.471(4) . 51
Zn2B Cr20 Zn2B 109.5 28 51
Zn2B Cr20 Zn2B 109.471(1) . 74
Zn2B Cr20 Zn2B 109.471(2) 28 74
Zn2B Cr20 Zn2B 109.5 51 74
Zn2B Cr20 Zn21 9.0(4) . 9
Zn2B Cr20 Zn21 100.5(4) 28 9
Zn2B Cr20 Zn21 113.77(18) 51 9
Zn2B Cr20 Zn21 113.77(18) 74 9
Zn2B Cr20 Zn21 9.0(4) . 5
Zn2B Cr20 Zn21 113.77(18) 28 5
Zn2B Cr20 Zn21 113.77(18) 51 5
Zn2B Cr20 Zn21 100.5(4) 74 5
Zn21 Cr20 Zn21 15.6(7) 9 5
Zn2B Cr20 Zn21 9.0(4) . .
Zn2B Cr20 Zn21 113.77(18) 28 .
Zn2B Cr20 Zn21 100.5(4) 51 .
Zn2B Cr20 Zn21 113.77(18) 74 .
Zn21 Cr20 Zn21 15.6(7) 9 .
Zn21 Cr20 Zn21 15.6(7) 5 .
Zn2B Cr20 Zn21 113.77(17) . 84
Zn2B Cr20 Zn21 113.77(17) 28 84
Zn2B Cr20 Zn21 100.5(4) 51 84
Zn2B Cr20 Zn21 9.0(4) 74 84
Zn21 Cr20 Zn21 119.2(4) 9 84
Zn21 Cr20 Zn21 104.9(2) 5 84
Zn21 Cr20 Zn21 116.8(2) . 84
Zn2B Cr20 Zn21 113.77(17) . 58
Zn2B Cr20 Zn21 113.77(17) 28 58
Zn2B Cr20 Zn21 9.0(4) 51 58
Zn2B Cr20 Zn21 100.5(4) 74 58
Zn21 Cr20 Zn21 119.2(4) 9 58
Zn21 Cr20 Zn21 116.8(2) 5 58
Zn21 Cr20 Zn21 104.9(2) . 58
Zn21 Cr20 Zn21 91.5(8) 84 58
Zn2B Cr20 Zn21 113.77(18) . 56
Zn2B Cr20 Zn21 100.5(4) 28 56
Zn2B Cr20 Zn21 9.0(4) 51 56
Zn2B Cr20 Zn21 113.77(17) 74 56
Zn21 Cr20 Zn21 116.8(2) 9 56
Zn21 Cr20 Zn21 119.2(4) 5 56
Zn21 Cr20 Zn21 104.9(2) . 56
Zn21 Cr20 Zn21 104.9(2) 84 56
Zn21 Cr20 Zn21 15.6(7) 58 56
Zn2B Cr20 Zn21 113.77(17) . 74
Zn2B Cr20 Zn21 100.5(4) 28 74
Zn2B Cr20 Zn21 113.77(17) 51 74
Zn2B Cr20 Zn21 9.0(4) 74 74
Zn21 Cr20 Zn21 116.8(2) 9 74
Zn21 Cr20 Zn21 104.9(2) 5 74
Zn21 Cr20 Zn21 119.2(4) . 74
Zn21 Cr20 Zn21 15.6(7) 84 74
Zn21 Cr20 Zn21 104.9(2) 58 74
Zn21 Cr20 Zn21 116.8(2) 56 74
Zn2B Cr20 Zn21 113.77(18) . 30
Zn2B Cr20 Zn21 9.0(4) 28 30
Zn2B Cr20 Zn21 100.5(4) 51 30
Zn2B Cr20 Zn21 113.77(17) 74 30
Zn21 Cr20 Zn21 104.9(2) 9 30
Zn21 Cr20 Zn21 119.2(4) 5 30
Zn21 Cr20 Zn21 116.8(2) . 30
Zn21 Cr20 Zn21 116.8(2) 84 30
Zn21 Cr20 Zn21 104.9(2) 58 30
Zn21 Cr20 Zn21 91.5(8) 56 30
Zn21 Cr20 Zn21 104.9(2) 74 30
Zn21 Zn2B Zn21 59(5) 9 5
Zn21 Zn2B Zn21 59(5) 9 .
Zn21 Zn2B Zn21 59(5) 5 .
Zn21 Zn2B Zn24 104(3) 9 84
Zn21 Zn2B Zn24 52.5(16) 5 84
Zn21 Zn2B Zn24 104(3) . 84
Zn21 Zn2B Zn24 104(3) 9 56
Zn21 Zn2B Zn24 104(3) 5 56
Zn21 Zn2B Zn24 52.5(16) . 56
Zn24 Zn2B Zn24 119.7(3) 84 56
Zn21 Zn2B Zn24 52.5(16) 9 28
Zn21 Zn2B Zn24 104(3) 5 28
Zn21 Zn2B Zn24 104(3) . 28
Zn24 Zn2B Zn24 119.7(3) 84 28
Zn24 Zn2B Zn24 119.7(3) 56 28
Zn21 Zn2B Cr20 145(3) 9 .
Zn21 Zn2B Cr20 145(3) 5 .
Zn21 Zn2B Cr20 145(3) . .
Zn24 Zn2B Cr20 92.9(16) 84 .
Zn24 Zn2B Cr20 92.9(16) 56 .
Zn24 Zn2B Cr20 92.9(16) 28 .
Zn21 Zn2B Zn26 109.3(14) 9 35
Zn21 Zn2B Zn26 69.0(19) 5 35
Zn21 Zn2B Zn26 124(3) . 35
Zn24 Zn2B Zn26 20.9(5) 84 35
Zn24 Zn2B Zn26 133.7(7) 56 35
Zn24 Zn2B Zn26 106.0(6) 28 35
Cr20 Zn2B Zn26 77.4(13) . 35
Zn21 Zn2B Zn26 124(3) 9 58
Zn21 Zn2B Zn26 69.0(19) 5 58
Zn21 Zn2B Zn26 109.3(14) . 58
Zn24 Zn2B Zn26 20.9(5) 84 58
Zn24 Zn2B Zn26 106.0(6) 56 58
Zn24 Zn2B Zn26 133.7(7) 28 58
Cr20 Zn2B Zn26 77.4(13) . 58
Zn26 Zn2B Zn26 27.7(9) 35 58
Zn21 Zn2B Zn26 124(3) 9 79
Zn21 Zn2B Zn26 109.3(14) 5 79
Zn21 Zn2B Zn26 69.0(19) . 79
Zn24 Zn2B Zn26 106.0(6) 84 79
Zn24 Zn2B Zn26 20.9(5) 56 79
Zn24 Zn2B Zn26 133.7(7) 28 79
Cr20 Zn2B Zn26 77.4(13) . 79
Zn26 Zn2B Zn26 115.4(9) 35 79
Zn26 Zn2B Zn26 88.8(11) 58 79
Zn21 Zn2B Zn26 109.3(14) 9 30
Zn21 Zn2B Zn26 124(3) 5 30
Zn21 Zn2B Zn26 69.0(19) . 30
Zn24 Zn2B Zn26 133.7(7) 84 30
Zn24 Zn2B Zn26 20.9(5) 56 30
Zn24 Zn2B Zn26 106.0(6) 28 30
Cr20 Zn2B Zn26 77.4(13) . 30
Zn26 Zn2B Zn26 139.8(17) 35 30
Zn26 Zn2B Zn26 115.4(9) 58 30
Zn26 Zn2B Zn26 27.7(9) 79 30
Zn21 Zn2B Zn26 69.0(19) 9 51
Zn21 Zn2B Zn26 124(3) 5 51
Zn21 Zn2B Zn26 109.3(14) . 51
Zn24 Zn2B Zn26 133.7(7) 84 51
Zn24 Zn2B Zn26 106.0(6) 56 51
Zn24 Zn2B Zn26 20.9(5) 28 51
Cr20 Zn2B Zn26 77.4(13) . 51
Zn26 Zn2B Zn26 115.4(9) 35 51
Zn26 Zn2B Zn26 139.8(17) 58 51
Zn26 Zn2B Zn26 115.4(9) 79 51
Zn26 Zn2B Zn26 88.8(11) 30 51
Zn21 Zn21 Zn21 60.000(6) 9 5
Zn21 Zn21 Zn2B 61(3) 9 .
Zn21 Zn21 Zn2B 61(3) 5 .
Zn21 Zn21 Zn24 144.4(3) 9 56
Zn21 Zn21 Zn24 144.4(3) 5 56
Zn2B Zn21 Zn24 104(3) . 56
Zn21 Zn21 Zn24 80.2(4) 9 84
Zn21 Zn21 Zn24 24.2(3) 5 84
Zn2B Zn21 Zn24 56.3(17) . 84
Zn24 Zn21 Zn24 120.2(4) 56 84
Zn21 Zn21 Zn24 24.2(3) 9 28
Zn21 Zn21 Zn24 80.2(4) 5 28
Zn2B Zn21 Zn24 56.3(17) . 28
Zn24 Zn21 Zn24 120.2(4) 56 28
Zn24 Zn21 Zn24 95.8(8) 84 28
Zn21 Zn21 Zn26 146.7(5) 9 79
Zn21 Zn21 Zn26 125.4(6) 5 79
Zn2B Zn21 Zn26 92(3) . 79
Zn24 Zn21 Zn26 19.1(5) 56 79
Zn24 Zn21 Zn26 101.3(6) 84 79
Zn24 Zn21 Zn26 125.2(5) 28 79
Zn21 Zn21 Zn26 125.4(6) 9 30
Zn21 Zn21 Zn26 146.7(5) 5 30
Zn2B Zn21 Zn26 92(3) . 30
Zn24 Zn21 Zn26 19.1(5) 56 30
Zn24 Zn21 Zn26 125.2(5) 84 30
Zn24 Zn21 Zn26 101.3(6) 28 30
Zn26 Zn21 Zn26 29.7(10) 79 30
Zn21 Zn21 Au23 144.83(17) 9 30
Zn21 Zn21 Au23 144.83(17) 5 30
Zn2B Zn21 Au23 105(3) . 30
Zn24 Zn21 Au23 0.9(4) 56 30
Zn24 Zn21 Au23 120.7(3) 84 30
Zn24 Zn21 Au23 120.7(3) 28 30
Zn26 Zn21 Au23 19.6(5) 79 30
Zn26 Zn21 Au23 19.6(5) 30 30
Zn21 Zn21 Zn23 144.83(17) 9 30
Zn21 Zn21 Zn23 144.83(17) 5 30
Zn2B Zn21 Zn23 105(3) . 30
Zn24 Zn21 Zn23 0.9(4) 56 30
Zn24 Zn21 Zn23 120.7(3) 84 30
Zn24 Zn21 Zn23 120.7(3) 28 30
Zn26 Zn21 Zn23 19.6(5) 79 30
Zn26 Zn21 Zn23 19.6(5) 30 30
Au23 Zn21 Zn23 0.0 30 30
Zn21 Zn21 Zn25 131.3(3) 9 30
Zn21 Zn21 Zn25 82.0(4) 5 30
Zn2B Zn21 Zn25 126.8(5) . 30
Zn24 Zn21 Zn25 84.1(6) 56 30
Zn24 Zn21 Zn25 73.78(18) 84 30
Zn24 Zn21 Zn25 155.1(6) 28 30
Zn26 Zn21 Zn25 79.5(6) 79 30
Zn26 Zn21 Zn25 103.1(8) 30 30
Au23 Zn21 Zn25 83.5(5) 30 30
Zn23 Zn21 Zn25 83.5(5) 30 30
Zn21 Zn21 Zn25 82.0(4) 9 74
Zn21 Zn21 Zn25 131.3(3) 5 74
Zn2B Zn21 Zn25 126.8(5) . 74
Zn24 Zn21 Zn25 84.1(6) 56 74
Zn24 Zn21 Zn25 155.1(6) 84 74
Zn24 Zn21 Zn25 73.78(18) 28 74
Zn26 Zn21 Zn25 103.1(8) 79 74
Zn26 Zn21 Zn25 79.5(6) 30 74
Au23 Zn21 Zn25 83.5(5) 30 74
Zn23 Zn21 Zn25 83.5(5) 30 74
Zn25 Zn21 Zn25 106.2(5) 30 74
Zn26 Zn22 Zn26 105.8(5) 84 56
Zn26 Zn22 Zn26 105.8(5) 84 28
Zn26 Zn22 Zn26 105.8(5) 56 28
Zn26 Zn22 Zn24 16.2(3) 84 35
Zn26 Zn22 Zn24 114.9(4) 56 35
Zn26 Zn22 Zn24 90.1(3) 28 35
Zn26 Zn22 Zn24 16.2(3) 84 58
Zn26 Zn22 Zn24 90.1(3) 56 58
Zn26 Zn22 Zn24 114.9(4) 28 58
Zn24 Zn22 Zn24 30.4(5) 35 58
Zn26 Zn22 Zn24 90.1(3) 84 79
Zn26 Zn22 Zn24 16.2(3) 56 79
Zn26 Zn22 Zn24 114.9(4) 28 79
Zn24 Zn22 Zn24 100.6(2) 35 79
Zn24 Zn22 Zn24 74.2(5) 58 79
Zn26 Zn22 Zn24 114.9(4) 84 30
Zn26 Zn22 Zn24 16.2(3) 56 30
Zn26 Zn22 Zn24 90.1(3) 28 30
Zn24 Zn22 Zn24 120.0(4) 35 30
Zn24 Zn22 Zn24 100.6(2) 58 30
Zn24 Zn22 Zn24 30.4(5) 79 30
Zn26 Zn22 Zn24 114.9(4) 84 51
Zn26 Zn22 Zn24 90.1(3) 56 51
Zn26 Zn22 Zn24 16.2(3) 28 51
Zn24 Zn22 Zn24 100.6(2) 35 51
Zn24 Zn22 Zn24 120.0(4) 58 51
Zn24 Zn22 Zn24 100.6(2) 79 51
Zn24 Zn22 Zn24 74.2(5) 30 51
Zn26 Zn22 Zn24 90.1(3) 84 74
Zn26 Zn22 Zn24 114.9(4) 56 74
Zn26 Zn22 Zn24 16.2(3) 28 74
Zn24 Zn22 Zn24 74.2(5) 35 74
Zn24 Zn22 Zn24 100.6(2) 58 74
Zn24 Zn22 Zn24 120.0(4) 79 74
Zn24 Zn22 Zn24 100.6(2) 30 74
Zn24 Zn22 Zn24 30.4(5) 51 74
Zn26 Zn22 Zn15 64.0(4) 84 .
Zn26 Zn22 Zn15 127.1(3) 56 .
Zn26 Zn22 Zn15 127.1(3) 28 .
Zn24 Zn22 Zn15 70.30(18) 35 .
Zn24 Zn22 Zn15 70.30(18) 58 .
Zn24 Zn22 Zn15 116.8(2) 79 .
Zn24 Zn22 Zn15 142.5(2) 30 .
Zn24 Zn22 Zn15 142.5(2) 51 .
Zn24 Zn22 Zn15 116.8(2) 74 .
Zn26 Zn22 Zn15 127.1(3) 84 5
Zn26 Zn22 Zn15 127.1(3) 56 5
Zn26 Zn22 Zn15 64.0(4) 28 5
Zn24 Zn22 Zn15 116.8(2) 35 5
Zn24 Zn22 Zn15 142.5(2) 58 5
Zn24 Zn22 Zn15 142.5(2) 79 5
Zn24 Zn22 Zn15 116.8(2) 30 5
Zn24 Zn22 Zn15 70.30(18) 51 5
Zn24 Zn22 Zn15 70.30(18) 74 5
Zn15 Zn22 Zn15 81.47(7) . 5
Zn26 Zn22 Zn15 127.1(3) 84 9
Zn26 Zn22 Zn15 64.0(4) 56 9
Zn26 Zn22 Zn15 127.1(3) 28 9
Zn24 Zn22 Zn15 142.5(2) 35 9
Zn24 Zn22 Zn15 116.8(2) 58 9
Zn24 Zn22 Zn15 70.30(18) 79 9
Zn24 Zn22 Zn15 70.30(18) 30 9
Zn24 Zn22 Zn15 116.8(2) 51 9
Zn24 Zn22 Zn15 142.5(2) 74 9
Zn15 Zn22 Zn15 81.47(7) . 9
Zn15 Zn22 Zn15 81.47(7) 5 9
Zn26 Zn23 Zn26 88(2) . 28
Zn26 Zn23 Zn24 64.3(6) . 51
Zn26 Zn23 Zn24 64.3(6) 28 51
Zn26 Zn23 Zn24 64.3(6) . 74
Zn26 Zn23 Zn24 64.3(6) 28 74
Zn24 Zn23 Zn24 106.1(13) 51 74
Zn26 Zn23 Zn21 65.3(5) . 84
Zn26 Zn23 Zn21 65.3(5) 28 84
Zn24 Zn23 Zn21 1.5(7) 51 84
Zn24 Zn23 Zn21 107.6(7) 74 84
Zn26 Zn23 Zn21 65.3(5) . 58
Zn26 Zn23 Zn21 65.3(5) 28 58
Zn24 Zn23 Zn21 107.6(7) 51 58
Zn24 Zn23 Zn21 1.5(7) 74 58
Zn21 Zn23 Zn21 109.1(6) 84 58
Zn26 Zn23 Zn35 123.4(7) . 79
Zn26 Zn23 Zn35 123.4(7) 28 79
Zn24 Zn23 Zn35 167.2(6) 51 79
Zn24 Zn23 Zn35 86.8(6) 74 79
Zn21 Zn23 Zn35 165.6(3) 84 79
Zn21 Zn23 Zn35 85.3(3) 58 79
Zn26 Zn23 Zn35 123.4(7) . 56
Zn26 Zn23 Zn35 123.4(7) 28 56
Zn24 Zn23 Zn35 86.8(6) 51 56
Zn24 Zn23 Zn35 167.2(6) 74 56
Zn21 Zn23 Zn35 85.3(3) 84 56
Zn21 Zn23 Zn35 165.6(3) 58 56
Zn35 Zn23 Zn35 80.39(8) 79 56
Zn26 Zn23 Zn2B 55.9(10) . 74
Zn26 Zn23 Zn2B 55.9(10) 28 74
Zn24 Zn23 Zn2B 14.1(13) 51 74
Zn24 Zn23 Zn2B 92.0(13) 74 74
Zn21 Zn23 Zn2B 15.6(9) 84 74
Zn21 Zn23 Zn2B 93.5(14) 58 74
Zn35 Zn23 Zn2B 178.8(11) 79 74
Zn35 Zn23 Zn2B 100.8(11) 56 74
Zn26 Zn23 Zn2B 55.9(10) . 51
Zn26 Zn23 Zn2B 55.9(10) 28 51
Zn24 Zn23 Zn2B 92.0(13) 51 51
Zn24 Zn23 Zn2B 14.1(13) 74 51
Zn21 Zn23 Zn2B 93.5(14) 84 51
Zn21 Zn23 Zn2B 15.6(9) 58 51
Zn35 Zn23 Zn2B 100.8(11) 79 51
Zn35 Zn23 Zn2B 178.8(11) 56 51
Zn2B Zn23 Zn2B 78(2) 74 51
Zn26 Zn23 Zn15 157.5(12) . 5
Zn26 Zn23 Zn15 69.9(12) 28 5
Zn24 Zn23 Zn15 104.0(2) 51 5
Zn24 Zn23 Zn15 104.0(2) 74 5
Zn21 Zn23 Zn15 103.49(11) 84 5
Zn21 Zn23 Zn15 103.49(11) 58 5
Zn35 Zn23 Zn15 72.10(4) 79 5
Zn35 Zn23 Zn15 72.10(4) 56 5
Zn2B Zn23 Zn15 108.2(3) 74 5
Zn2B Zn23 Zn15 108.2(3) 51 5
Zn26 Zn23 Zn15 69.9(12) . 30
Zn26 Zn23 Zn15 157.5(12) 28 30
Zn24 Zn23 Zn15 104.0(2) 51 30
Zn24 Zn23 Zn15 104.0(2) 74 30
Zn21 Zn23 Zn15 103.49(11) 84 30
Zn21 Zn23 Zn15 103.49(11) 58 30
Zn35 Zn23 Zn15 72.10(4) 79 30
Zn35 Zn23 Zn15 72.10(4) 56 30
Zn2B Zn23 Zn15 108.2(3) 74 30
Zn2B Zn23 Zn15 108.2(3) 51 30
Zn15 Zn23 Zn15 132.56(10) 5 30
Au23 Zn24 Zn23 0.0(2) 74 74
Au23 Zn24 Zn26 54.2(12) 74 51
Zn23 Zn24 Zn26 54.2(12) 74 51
Au23 Zn24 Zn26 54.2(12) 74 74
Zn23 Zn24 Zn26 54.2(12) 74 74
Zn26 Zn24 Zn26 77(2) 51 74
Au23 Zn24 Zn24 37.0(6) 74 28
Zn23 Zn24 Zn24 37.0(6) 74 28
Zn26 Zn24 Zn24 38.8(11) 51 28
Zn26 Zn24 Zn24 38.8(11) 74 28
Au23 Zn24 Zn21 177.6(12) 74 35
Zn23 Zn24 Zn21 177.6(12) 74 35
Zn26 Zn24 Zn21 127.3(12) 51 35
Zn26 Zn24 Zn21 127.3(12) 74 35
Zn24 Zn24 Zn21 145.4(6) 28 35
Au23 Zn24 Zn2B 159.4(19) 74 28
Zn23 Zn24 Zn2B 159.4(19) 74 28
Zn26 Zn24 Zn2B 111.3(17) 51 28
Zn26 Zn24 Zn2B 111.3(17) 74 28
Zn24 Zn24 Zn2B 122.4(16) 28 28
Zn21 Zn24 Zn2B 23.0(12) 35 28
Au23 Zn24 Zn21 169.6(5) 74 30
Zn23 Zn24 Zn21 169.6(5) 74 30
Zn26 Zn24 Zn21 115.9(12) 51 30
Zn26 Zn24 Zn21 130.5(13) 74 30
Zn24 Zn24 Zn21 138.5(3) 28 30
Zn21 Zn24 Zn21 11.5(5) 35 30
Zn2B Zn24 Zn21 19.7(12) 28 30
Au23 Zn24 Zn21 169.6(5) 74 28
Zn23 Zn24 Zn21 169.6(5) 74 28
Zn26 Zn24 Zn21 130.5(13) 51 28
Zn26 Zn24 Zn21 115.9(12) 74 28
Zn24 Zn24 Zn21 138.5(3) 28 28
Zn21 Zn24 Zn21 11.5(5) 35 28
Zn2B Zn24 Zn21 19.7(12) 28 28
Zn21 Zn24 Zn21 19.6(8) 30 28
Au23 Zn24 Zn35 74.0(6) 74 5
Zn23 Zn24 Zn35 74.0(6) 74 5
Zn26 Zn24 Zn35 109.7(12) 51 5
Zn26 Zn24 Zn35 109.7(12) 74 5
Zn24 Zn24 Zn35 110.9(2) 28 5
Zn21 Zn24 Zn35 103.6(7) 35 5
Zn2B Zn24 Zn35 126.7(17) 28 5
Zn21 Zn24 Zn35 109.3(5) 30 5
Zn21 Zn24 Zn35 109.3(5) 28 5
Au23 Zn24 Zn22 92.7(4) 74 51
Zn23 Zn24 Zn22 92.7(4) 74 51
Zn26 Zn24 Zn22 107.9(13) 51 51
Zn26 Zn24 Zn22 39.5(11) 74 51
Zn24 Zn24 Zn22 74.8(2) 28 51
Zn21 Zn24 Zn22 88.5(4) 35 51
Zn2B Zn24 Zn22 77.3(8) 28 51
Zn21 Zn24 Zn22 94.1(5) 30 51
Zn21 Zn24 Zn22 77.0(4) 28 51
Zn35 Zn24 Zn22 119.54(19) 5 51
Au23 Zn24 Zn22 92.7(4) 74 74
Zn23 Zn24 Zn22 92.7(4) 74 74
Zn26 Zn24 Zn22 39.5(11) 51 74
Zn26 Zn24 Zn22 107.9(13) 74 74
Zn24 Zn24 Zn22 74.8(2) 28 74
Zn21 Zn24 Zn22 88.5(4) 35 74
Zn2B Zn24 Zn22 77.3(8) 28 74
Zn21 Zn24 Zn22 77.0(4) 30 74
Zn21 Zn24 Zn22 94.1(5) 28 74
Zn35 Zn24 Zn22 119.54(19) 5 74
Zn22 Zn24 Zn22 119.8(4) 51 74
Zn23 Zn26 Zn24 61.5(13) . 51
Zn23 Zn26 Zn24 61.5(13) . 74
Zn24 Zn26 Zn24 102(2) 51 74
Zn23 Zn26 Zn26 46.2(11) . 28
Zn24 Zn26 Zn26 51.4(11) 51 28
Zn24 Zn26 Zn26 51.4(11) 74 28
Zn23 Zn26 Zn22 165.6(16) . 28
Zn24 Zn26 Zn22 124.3(12) 51 28
Zn24 Zn26 Zn22 124.3(12) 74 28
Zn26 Zn26 Zn22 148.2(4) 28 28
Zn23 Zn26 Zn21 95.1(8) . 84
Zn24 Zn26 Zn21 33.7(9) 51 84
Zn24 Zn26 Zn21 124.0(15) 74 84
Zn26 Zn26 Zn21 75.2(5) 28 84
Zn22 Zn26 Zn21 91.3(6) 28 84
Zn23 Zn26 Zn21 95.1(8) . 58
Zn24 Zn26 Zn21 124.0(15) 51 58
Zn24 Zn26 Zn21 33.7(9) 74 58
Zn26 Zn26 Zn21 75.2(5) 28 58
Zn22 Zn26 Zn21 91.3(6) 28 58
Zn21 Zn26 Zn21 126.6(10) 84 58
Zn23 Zn26 Zn2B 107.5(12) . 74
Zn24 Zn26 Zn2B 47.7(13) 51 74
Zn24 Zn26 Zn2B 117.1(16) 74 74
Zn26 Zn26 Zn2B 76.2(5) 28 74
Zn22 Zn26 Zn2B 82.1(7) 28 74
Zn21 Zn26 Zn2B 18.7(9) 84 74
Zn21 Zn26 Zn2B 110.3(16) 58 74
Zn23 Zn26 Zn2B 107.5(12) . 51
Zn24 Zn26 Zn2B 117.1(16) 51 51
Zn24 Zn26 Zn2B 47.7(13) 74 51
Zn26 Zn26 Zn2B 76.2(5) 28 51
Zn22 Zn26 Zn2B 82.1(7) 28 51
Zn21 Zn26 Zn2B 110.3(16) 84 51
Zn21 Zn26 Zn2B 18.7(9) 58 51
Zn2B Zn26 Zn2B 93(2) 74 51
Zn23 Zn26 Zn15 93.5(12) . 30
Zn24 Zn26 Zn15 115.8(12) 51 30
Zn24 Zn26 Zn15 115.8(12) 74 30
Zn26 Zn26 Zn15 139.7(4) 28 30
Zn22 Zn26 Zn15 72.1(5) 28 30
Zn21 Zn26 Zn15 115.7(5) 84 30
Zn21 Zn26 Zn15 115.7(5) 58 30
Zn2B Zn26 Zn15 126.9(9) 74 30
Zn2B Zn26 Zn15 126.9(9) 51 30
Zn23 Zn26 Zn21 108.0(7) . 51
Zn24 Zn26 Zn21 131.4(15) 51 51
Zn24 Zn26 Zn21 46.6(9) 74 51
Zn26 Zn26 Zn21 85.9(5) 28 51
Zn22 Zn26 Zn21 78.4(5) 28 51
Zn21 Zn26 Zn21 124.9(9) 84 51
Zn21 Zn26 Zn21 13.0(6) 58 51
Zn2B Zn26 Zn21 106.8(15) 74 51
Zn2B Zn26 Zn21 15.3(8) 51 51
Zn15 Zn26 Zn21 112.0(5) 30 51
Zn21 Zn25 Zn21 16.0(8) 84 74
Zn21 Zn25 Zn13 161.8(2) 84 9
Zn21 Zn25 Zn13 161.8(2) 74 9
Zn21 Zn25 Zn32 62.56(15) 84 74
Zn21 Zn25 Zn32 62.56(15) 74 74
Zn13 Zn25 Zn32 134.19(9) 9 74
Zn21 Zn25 Zn15 96.2(3) 84 5
Zn21 Zn25 Zn15 106.6(3) 74 5
Zn13 Zn25 Zn15 66.40(6) 9 5
Zn32 Zn25 Zn15 138.49(5) 74 5
Zn21 Zn25 Zn15 106.6(3) 84 9
Zn21 Zn25 Zn15 96.2(3) 74 9
Zn13 Zn25 Zn15 66.40(6) 9 9
Zn32 Zn25 Zn15 138.49(5) 74 9
Zn15 Zn25 Zn15 79.69(8) 5 9
Zn21 Zn25 Zn24 45.4(4) 84 30
Zn21 Zn25 Zn24 31.2(4) 74 30
Zn13 Zn25 Zn24 132.40(19) 9 30
Zn32 Zn25 Zn24 83.29(18) 74 30
Zn15 Zn25 Zn24 107.45(16) 5 30
Zn15 Zn25 Zn24 66.10(18) 9 30
Zn21 Zn25 Zn24 31.2(4) 84 51
Zn21 Zn25 Zn24 45.4(4) 74 51
Zn13 Zn25 Zn24 132.40(19) 9 51
Zn32 Zn25 Zn24 83.29(18) 74 51
Zn15 Zn25 Zn24 66.10(18) 5 51
Zn15 Zn25 Zn24 107.45(16) 9 51
Zn24 Zn25 Zn24 66.8(4) 30 51
Zn21 Zn25 Zn34 113.5(2) 84 3_556
Zn21 Zn25 Zn34 121.5(2) 74 3_556
Zn13 Zn25 Zn34 76.75(7) 9 3_556
Zn32 Zn25 Zn34 62.59(5) 74 3_556
Zn15 Zn25 Zn34 100.86(4) 5 3_556
Zn15 Zn25 Zn34 139.56(8) 9 3_556
Zn24 Zn25 Zn34 145.72(17) 30 3_556
Zn24 Zn25 Zn34 109.54(16) 51 3_556
Zn21 Zn25 Zn34 121.5(2) 84 4_556
Zn21 Zn25 Zn34 113.5(2) 74 4_556
Zn13 Zn25 Zn34 76.75(7) 9 4_556
Zn32 Zn25 Zn34 62.59(5) 74 4_556
Zn15 Zn25 Zn34 139.56(8) 5 4_556
Zn15 Zn25 Zn34 100.86(4) 9 4_556
Zn24 Zn25 Zn34 109.54(16) 30 4_556
Zn24 Zn25 Zn34 145.72(17) 51 4_556
Zn34 Zn25 Zn34 53.09(5) 3_556 4_556
Zn21 Zn25 Zn35 72.4(4) 84 56
Zn21 Zn25 Zn35 87.9(4) 74 56
Zn13 Zn25 Zn35 103.12(4) 9 56
Zn32 Zn25 Zn35 73.98(4) 74 56
Zn15 Zn25 Zn35 65.38(4) 5 56
Zn15 Zn25 Zn35 144.44(6) 9 56
Zn24 Zn25 Zn35 117.1(2) 30 56
Zn24 Zn25 Zn35 53.10(17) 51 56
Zn34 Zn25 Zn35 58.74(4) 3_556 56
Zn34 Zn25 Zn35 109.82(5) 4_556 56
Zn21 Zn25 Zn35 87.9(4) 84 35
Zn21 Zn25 Zn35 72.4(4) 74 35
Zn13 Zn25 Zn35 103.12(4) 9 35
Zn32 Zn25 Zn35 73.98(4) 74 35
Zn15 Zn25 Zn35 144.44(6) 5 35
Zn15 Zn25 Zn35 65.38(4) 9 35
Zn24 Zn25 Zn35 53.10(17) 30 35
Zn24 Zn25 Zn35 117.1(2) 51 35
Zn34 Zn25 Zn35 109.82(5) 3_556 35
Zn34 Zn25 Zn35 58.74(4) 4_556 35
Zn35 Zn25 Zn35 147.46(7) 56 35
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Zn10 Zn11 1.735(3) .
Zn10 Zn11 1.735(3) 4
Zn10 Zn11 1.735(3) 2
Zn10 Zn11 1.735(3) 3
Zn10 Au12 2.7548(5) 1_444
Zn10 Au12 2.7548(5) 4_466
Zn10 Au12 2.7548(5) 2_664
Zn10 Au12 2.7548(5) 3_646
Zn11 Zn13 2.646(3) 9
Zn11 Zn13 2.646(3) 5
Zn11 Zn13 2.646(3) .
Zn11 Zn15 2.704(3) .
Zn11 Zn15 2.704(3) 9
Zn11 Zn15 2.704(3) 5
Zn11 Au12 2.7226(11) 2_664
Zn11 Au12 2.7226(11) 3_646
Zn11 Au12 2.7226(11) 4_466
Zn11 Zn11 2.833(5) 4
Zn11 Zn11 2.833(5) 2
Au12 Zn45 2.5966(12) 10_656
Au12 Zn45 2.5966(12) 6_566
Au12 Zn45 2.5966(12) 2_665
Au12 Zn15 2.7095(12) 2_666
Au12 Zn15 2.7095(12) 10_666
Au12 Zn15 2.7095(12) 6_666
Au12 Zn11 2.7226(11) 2_666
Au12 Zn11 2.7226(11) 3_666
Au12 Zn11 2.7226(11) 4_666
Au12 Zn10 2.7548(5) 1_666
Au12 Zn13 2.787(2) 2_666
Au12 Zn13 2.787(2) 6_666
Zn13 Zn25 2.643(3) 5
Zn13 Zn25 2.643(3) 6
Zn13 Zn11 2.646(3) 4
Zn13 Au12 2.787(2) 2_664
Zn13 Au12 2.787(2) 3_646
Zn13 Zn45 2.9241(16) 8_655
Zn13 Zn45 2.9241(16) 7_655
Zn13 Zn15 2.9244(9) 4
Zn13 Zn15 2.9244(9) 11
Zn13 Zn15 2.9244(9) 9
Zn13 Zn15 2.9244(9) .
Zn15 Zn26 2.502(15) 84
Zn15 Zn22 2.648(2) .
Zn15 Au23 2.6592(15) 9
Zn15 Zn23 2.6592(15) 9
Zn15 Zn25 2.6966(11) 9
Zn15 Zn25 2.6966(11) 5
Zn15 Au12 2.7095(12) 2_664
Zn15 Zn45 2.8530(13) 8_655
Zn15 Zn45 2.8530(13) 11_565
Zn15 Zn13 2.9244(9) 5
Cr42 Zn45 2.5585(12) 57
Cr42 Zn45 2.5585(12) 29
Cr42 Zn45 2.5585(12) 73
Cr42 Zn34 2.611(2) 57
Cr42 Zn34 2.611(2) 29
Cr42 Zn34 2.611(2) 73
Cr42 Zn35 2.6308(14) 57
Cr42 Zn35 2.6308(14) 29
Cr42 Zn35 2.6308(14) 73
Cr42 Zn43 2.6323(18) 81
Cr42 Zn43 2.6323(18) 25
Cr42 Zn43 2.6323(18) 53
Zn43 Cr42 2.6323(18) 4_566
Zn43 Cr42 2.6323(18) 25_544
Zn43 Zn45 2.7461(11) 81_545
Zn43 Zn45 2.7461(11) 49_554
Zn43 Zn45 2.7461(11) 59_565
Zn43 Zn45 2.7461(11) 76_556
Zn43 Zn43 2.761(2) 10_656
Zn43 Zn43 2.761(2) 54_565
Zn43 Zn43 2.761(2) 57_554
Zn43 Zn43 2.761(2) 77_545
Zn43 Zn35 2.7756(19) 5
Zn43 Zn35 2.7756(19) 30
Zn45 Cr42 2.5585(12) 73_445
Zn45 Au12 2.5966(12) 2_665
Zn45 Zn34 2.7193(17) .
Zn45 Zn35 2.7245(10) 33_545
Zn45 Zn35 2.7245(10) 53_455
Zn45 Zn43 2.7461(11) 29_545
Zn45 Zn43 2.7461(11) 49_455
Zn45 Zn15 2.8530(13) 8_556
Zn45 Zn15 2.8530(13) 11_556
Zn45 Zn13 2.9241(16) 10_556
Zn45 Zn45 3.059(2) 11_566
Zn45 Zn45 3.059(2) 8_656
Zn30 Zn32 2.761(2) .
Zn30 Zn32 2.761(2) 4_566
Zn30 Zn32 2.761(2) 2_665
Zn30 Zn32 2.761(2) 3_656
Zn30 Zn34 3.0709(12) 57
Zn30 Zn34 3.0709(12) 73
Zn30 Zn34 3.0709(12) 29
Zn30 Zn34 3.0709(12) 58
Zn30 Zn34 3.0709(12) 74
Zn30 Zn34 3.0709(12) 30
Zn30 Zn34 3.0709(12) 60_565
Zn30 Zn34 3.0709(12) 31_655
Zn32 Zn25 2.6778(17) 58
Zn32 Zn25 2.6778(17) 30
Zn32 Zn25 2.6778(17) 74
Zn32 Zn21 2.691(7) .
Zn32 Zn21 2.691(7) 9
Zn32 Zn21 2.691(7) 5
Zn32 Zn34 2.8486(11) 59_565
Zn32 Zn34 2.8486(11) 60_565
Zn32 Zn34 2.8486(11) 32_655
Zn32 Zn34 2.8486(11) 31_655
Zn32 Zn34 2.8486(11) 75_556
Zn34 Zn34 2.504(2) 2
Zn34 Cr42 2.611(2) 73_445
Zn34 Zn34 2.713(2) 33_545
Zn34 Zn34 2.713(2) 53_455
Zn34 Zn35 2.7585(13) 33_545
Zn34 Zn35 2.7585(13) 53_455
Zn34 Zn25 2.8020(15) 4_556
Zn34 Zn25 2.8020(15) 3_556
Zn34 Zn32 2.8486(11) 75_546
Zn34 Zn32 2.8486(11) 76_456
Zn34 Zn30 3.0709(12) 73_445
Zn35 Au23 2.396(2) 58
Zn35 Zn23 2.396(2) 58
Zn35 Zn24 2.489(9) 9
Zn35 Cr42 2.6308(14) 73_445
Zn35 Zn45 2.7245(10) 33_545
Zn35 Zn45 2.7245(10) 53_455
Zn35 Zn34 2.7585(13) 33_545
Zn35 Zn34 2.7585(13) 53_455
Zn35 Zn43 2.7756(19) 9
Zn35 Zn25 2.8226(11) 35
Zn35 Zn25 2.8226(11) 56
Zn35 Zn26 2.885(14) 35
Cr20 Zn2B 1.95(5) .
Cr20 Zn2B 1.95(5) 28
Cr20 Zn2B 1.95(5) 51
Cr20 Zn2B 1.95(5) 74
Cr20 Zn21 2.562(10) 9
Cr20 Zn21 2.562(10) 5
Cr20 Zn21 2.562(10) .
Cr20 Zn21 2.562(10) 84
Cr20 Zn21 2.562(10) 58
Cr20 Zn21 2.562(10) 56
Cr20 Zn21 2.562(10) 74
Cr20 Zn21 2.562(10) 30
Zn2B Zn21 0.71(3) 9
Zn2B Zn21 0.71(3) 5
Zn2B Zn21 0.71(3) .
Zn2B Zn24 1.746(10) 84
Zn2B Zn24 1.746(10) 56
Zn2B Zn24 1.746(10) 28
Zn2B Zn26 2.198(15) 35
Zn2B Zn26 2.198(15) 58
Zn2B Zn26 2.198(15) 79
Zn2B Zn26 2.198(15) 30
Zn2B Zn26 2.198(15) 51
Zn21 Zn21 0.69(3) 9
Zn21 Zn21 0.69(3) 5
Zn21 Zn24 1.430(19) 56
Zn21 Zn24 2.036(16) 84
Zn21 Zn24 2.036(16) 28
Zn21 Zn26 2.054(15) 79
Zn21 Zn26 2.054(15) 30
Zn21 Au23 2.253(16) 30
Zn21 Zn23 2.253(16) 30
Zn21 Zn25 2.495(9) 30
Zn21 Zn25 2.495(9) 74
Zn22 Zn26 1.928(18) 84
Zn22 Zn26 1.928(18) 56
Zn22 Zn26 1.928(18) 28
Zn22 Zn24 2.503(5) 35
Zn22 Zn24 2.503(5) 58
Zn22 Zn24 2.503(5) 79
Zn22 Zn24 2.503(5) 30
Zn22 Zn24 2.503(5) 51
Zn22 Zn24 2.503(5) 74
Zn22 Zn15 2.648(2) 5
Zn22 Zn15 2.648(2) 9
Zn23 Zn26 0.760(17) .
Zn23 Zn26 0.760(17) 28
Zn23 Zn24 0.823(10) 51
Zn23 Zn24 0.823(10) 74
Zn23 Zn21 2.253(16) 84
Zn23 Zn21 2.253(16) 58
Zn23 Zn35 2.396(2) 79
Zn23 Zn35 2.396(2) 56
Zn23 Zn2B 2.532(4) 74
Zn23 Zn2B 2.532(4) 51
Zn23 Zn15 2.6592(15) 5
Zn23 Zn15 2.6592(15) 30
Zn24 Au23 0.823(10) 74
Zn24 Zn23 0.823(10) 74
Zn24 Zn26 0.843(11) 51
Zn24 Zn26 0.843(11) 74
Zn24 Zn24 1.31(2) 28
Zn24 Zn21 1.430(19) 35
Zn24 Zn2B 1.746(10) 28
Zn24 Zn21 2.036(16) 30
Zn24 Zn21 2.036(16) 28
Zn24 Zn35 2.489(9) 5
Zn24 Zn22 2.503(5) 51
Zn24 Zn22 2.503(5) 74
Zn26 Zn24 0.843(11) 51
Zn26 Zn24 0.843(11) 74
Zn26 Zn26 1.05(3) 28
Zn26 Zn22 1.928(18) 28
Zn26 Zn21 2.054(15) 84
Zn26 Zn21 2.054(15) 58
Zn26 Zn2B 2.198(15) 74
Zn26 Zn2B 2.198(15) 51
Zn26 Zn15 2.502(15) 30
Zn26 Zn21 2.521(12) 51
Zn25 Zn21 2.495(9) 84
Zn25 Zn21 2.495(9) 74
Zn25 Zn13 2.643(3) 9
Zn25 Zn32 2.6778(17) 74
Zn25 Zn15 2.6966(11) 5
Zn25 Zn15 2.6966(11) 9
Zn25 Zn24 2.745(7) 30
Zn25 Zn24 2.745(7) 51
Zn25 Zn34 2.8020(15) 3_556
Zn25 Zn34 2.8020(15) 4_556
Zn25 Zn35 2.8226(11) 56
Zn25 Zn35 2.8226(11) 35
